Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming for Hydrogen Production

*Itsaso Barbarias, Aitor Arregi, Maite Artetxe, Laura Santamaria, Gartzen Lopez, María Cortazar, Maider Amutio, Javier Bilbao and Martin Olazar*

## **Abstract**

This chapter summarizes the most recent results obtained in the plastic waste pyrolysis-reforming strategy for hydrogen production. An original two-reactor configuration consisting of a conical spouted bed reactor for the pyrolysis step and a fluidized bed reactor for the pyrolysis volatile reforming is proposed. The fundamental aspects and challenges of this joint process are discussed in detail, and the prospects for the full-scale implementation of this valorization route are assessed. Thus, the influence the main reforming parameters (temperature, space time and steam/ plastic ratio) have in the pyrolysis-reforming of HDPE on product yields and catalyst stability are reported. Moreover, the role played by plastic composition on process performance is also described by studying the influence of following polymers: high density polyethylene (HDPE), polypropylene (PP), polyethylene terephthalate (PET) and polystyrene (PS). The operating conditions used for the valorization of different plastics have been as follows: pyrolysis temperature of 500°C, reforming temperature of 700°C, space time of 16.7 gcatalyst min gplastic−1 and steam/plastic ratio of 4.

**Keywords:** hydrogen, pyrolysis, reforming, waste plastics, spouted bed

## **1. Introduction**

The current overall hydrogen production has reached a value of 7.7 EJ/year, and an increase to 10 EJ/year is expected by the year 2050 [1]. Hydrogen demand is mainly related to ammonia production (51%), oil refining (31%), methanol production (10%), and other uses (8%). Moreover, new fossil sources of lower quality than conventional oil are increasingly been used, but they require severe hydroprocessing for their upgrading. This is the case of oil sands, which surely will contribute to meeting the increasing requirements of hydrogen.

Approximately 96% of the world hydrogen produced is of fossil origin. Thus, 48% is produced from natural gas reforming, 30% from oil fractions and the remaining 18% by means of coal gasification [2]. Accordingly, only 4% is produced from renewable sources, such as water electrolysis.

The future of the hydrogen market is conditioned by the need to reduce CO2 emissions, which requires obtaining it from raw materials and renewable energy sources. The so-called hydrogen economy contemplates a future scenario in which this gas produced in a clean and economical way from a wide range of renewable sources would contribute to meeting the society's energy needs through combustion engines or preferably, by means of fuel cells, to a more efficient energy generation. This proposal would help to decentralize and diversify the energy system and reduce the current dependence on fossil fuels and air pollution [3].

In this scenario, the processes aimed at hydrogen production from biomass and waste are gaining growing attention [1, 4–6], with the thermochemical routes being those with best perspectives for their full scale implementation. Thus, hydrogen production from waste plastics has been mainly approached by means of steam gasification and pyrolysis-reforming processes [6].

Gasification allows for the conversion of waste plastics into a gaseous stream with varying contents of H2, CO, CO2, CH4 and N2 depending on process conditions and the gasifying agent used. The main advantage of gasification in relation to other thermochemical processes lies in its flexibility to valorize plastics of different composition or mixtures or plastics with other feedstocks. The main technologies for waste plastics gasification are those previously developed for biomass and coal gasification. It is to note that fluidized bed reactors have been widely used in the gasification of plastics [7–13]. However, these studies were mainly performed using air as fluidizing agent, so that the resulting gas has low hydrogen content and its main interest is restricted to energy production. The dual fluidized bed technology has been successfully applied to the steam gasification of plastics [13] and plastics mixtures with coal and biomass [14, 15]. The relevance of this technology is related with the fact that it allows overcoming the problems associated by the endothermic nature of the process. In spite of the promising results reported by Wilk et al. [13] in the gasification of different waste plastics, the high tar content in the syngas (above 100 g m<sup>−</sup><sup>3</sup> ) is a great challenge. However, waste plastic gasification has been scarcely studied in fixed bed reactors. Moreover, the results obtained are of preliminary nature as the reactors used are of laboratory scale and operate in batch regime [16–19]. Erkiaga et al. [20, 21] used the conical spouted bed reactor in the steam gasification of HDPE, and a hydrogen rich syngas was obtained with moderate tar contents. Moreover, this reactor design was also used subsequently in the co-gasification of HDPE and biomass (pine sawdust) with promising results [22]. The high temperatures attained in plasma reactors are also suitable for tar elimination, and this technology has therefore been proposed for the gasification of waste plastics [23, 24].

The hydrogen production from plastics via pyrolysis-reforming strategy has been recently proposed as an alternative to conventional gasification. The interest of this strategy lies in the fact that a tar free syngas is produced due to the high activity of the reforming catalyst. Moreover, the mild conditions in the reforming step and the physical separation of waste plastic impurities and the catalysts improve catalyst stability. Nevertheless, this strategy has been scarcely studied and the results reported were mainly obtained in lab scale units [6]. The studies by the team of Professor Williams [25–28] were carried out in a system in which pyrolysis is carried out in discontinuous regime in a fixed bed reactor and the volatiles are reformed in a second fixed bed. The reaction equipment used by the team of Professor Yoshikawa [29, 30] is a step forward, as it operates in continuous regime, although the use of fixed beds for pyrolysis and reforming can involve serious limitations for the process scale up. Czernik and French [31] made a step forward in this technology by studying the continuous pyrolysis and in-line reforming of polypropylene in a system of two in-line fluidized beds, with a commercial naphtha reforming catalyst. Erkiaga et al. [32] originally proposed a two-step reactor unit operating in continuous regime by

**71**

and, in fact, a 25 kg h<sup>−</sup><sup>1</sup>

PET and PS, are analyzed in this section.

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

quent studies to overcome the mentioned problems [33–36].

combining a spouted bed reactor for the plastic fast pyrolysis and a fixed bed for the catalytic steam reforming. However, the fixed bed reactor led to an excessive coke formation and severe operational problems subsequent to some minutes operation. Accordingly, the fixed bed reactor was replaced by a fluidized bed reactor in subse-

This chapter describes the main results obtained in the pyrolysis and in-line reforming of plastics in a system composed of a spouted bed for the pyrolysis step and a fluidized bed for the reforming one. Section 2 provides background information on the application of conical spouted beds to plastics pyrolysis. In addition, the results obtained in the pyrolysis of different plastics are also reported in this section, as long as the pyrolysis step product distribution is critical for the evaluation of the subsequent reforming step. Finally, Section 3 deals with the effect operating conditions (temperature, space time and S/P ratio) have on the reforming step performance. Moreover, the influence the polymer type in the feed to the pyrolysis step has on reforming step yields has also been evaluated. Thus, the interest of this chapter is centered on the maximization of hydrogen production under different conditions by treating plastics of different composition. Furthermore, one of the main challenges

of this process, as is catalyst stability, has also been approached in detail.

Pyrolysis (or thermal cracking) for the valorization of waste plastic is currently

The pyrolysis process is flexible and may treat plastic mixtures in the municipal solid waste, and those from automobile recycling, electronics and computers or construction, as well as mixtures of these materials with others (such as biomass) [41]. The requirements for scaling up and operation in continuous regime have led to the proposal of a significant number of technologies provided with very different reactors, such as fluidized beds, screw kilns, stirred or microwave reactors [37, 38]. Amongst these technologies, the fluidized bed reactor has been widely used because it ensures good heat and mass transfer, and therefore isothermal operation [42]. The main international reference in the development of this technology is known as the Hamburg process [43–45]. One of the main challenges in the pyrolysis of plastics is the sticky behavior of fused plastic particles, which causes agglomeration and subsequent defluidization in fluidized bed reactors [46]. The high heat transfer rates and vigorous cyclic movement of the particles in the conical spouted bed reactor, as well as the role of the spout to break up the agglomerates, are suitable features for continuous pyrolysis of plastics. Therefore, this technology allows operating below 500°C without defluidization problems [47]. Accordingly, the conical spouted bed has been successfully applied to the continuous pyrolysis of different polymeric materials [48–52]. Moreover, this technology has also been applied to the pyrolysis of biomass

pilot plant has been developed for this process [53, 54].

The main interest in analyzing the results obtained in the pyrolysis of the plastics lies in the fact that it constitutes the first step of the integrated pyrolysisreforming strategy, and therefore the volatile products of the pyrolysis process are the reactants of the catalytic reforming step. Consequently, it is essential to know the composition of the volatile stream leaving the pyrolysis step. Accordingly, the composition of the volatile stream for the pyrolysis of polyolefins (HDPE and PP),

receiving great attention, especially for addition polymers, which accounts for most plastics in the municipal solid waste stream. One of the main advantages of pyrolysis lies in its efficiency for the recovery of monomers and for the production of automotive and hydrogen fuels, with reduced emission of pollutants [37–40].

**2. Waste plastics pyrolysis in conical spouted beds**

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

combining a spouted bed reactor for the plastic fast pyrolysis and a fixed bed for the catalytic steam reforming. However, the fixed bed reactor led to an excessive coke formation and severe operational problems subsequent to some minutes operation. Accordingly, the fixed bed reactor was replaced by a fluidized bed reactor in subsequent studies to overcome the mentioned problems [33–36].

This chapter describes the main results obtained in the pyrolysis and in-line reforming of plastics in a system composed of a spouted bed for the pyrolysis step and a fluidized bed for the reforming one. Section 2 provides background information on the application of conical spouted beds to plastics pyrolysis. In addition, the results obtained in the pyrolysis of different plastics are also reported in this section, as long as the pyrolysis step product distribution is critical for the evaluation of the subsequent reforming step. Finally, Section 3 deals with the effect operating conditions (temperature, space time and S/P ratio) have on the reforming step performance. Moreover, the influence the polymer type in the feed to the pyrolysis step has on reforming step yields has also been evaluated. Thus, the interest of this chapter is centered on the maximization of hydrogen production under different conditions by treating plastics of different composition. Furthermore, one of the main challenges of this process, as is catalyst stability, has also been approached in detail.

## **2. Waste plastics pyrolysis in conical spouted beds**

Pyrolysis (or thermal cracking) for the valorization of waste plastic is currently receiving great attention, especially for addition polymers, which accounts for most plastics in the municipal solid waste stream. One of the main advantages of pyrolysis lies in its efficiency for the recovery of monomers and for the production of automotive and hydrogen fuels, with reduced emission of pollutants [37–40].

The pyrolysis process is flexible and may treat plastic mixtures in the municipal solid waste, and those from automobile recycling, electronics and computers or construction, as well as mixtures of these materials with others (such as biomass) [41]. The requirements for scaling up and operation in continuous regime have led to the proposal of a significant number of technologies provided with very different reactors, such as fluidized beds, screw kilns, stirred or microwave reactors [37, 38]. Amongst these technologies, the fluidized bed reactor has been widely used because it ensures good heat and mass transfer, and therefore isothermal operation [42]. The main international reference in the development of this technology is known as the Hamburg process [43–45].

One of the main challenges in the pyrolysis of plastics is the sticky behavior of fused plastic particles, which causes agglomeration and subsequent defluidization in fluidized bed reactors [46]. The high heat transfer rates and vigorous cyclic movement of the particles in the conical spouted bed reactor, as well as the role of the spout to break up the agglomerates, are suitable features for continuous pyrolysis of plastics. Therefore, this technology allows operating below 500°C without defluidization problems [47]. Accordingly, the conical spouted bed has been successfully applied to the continuous pyrolysis of different polymeric materials [48–52]. Moreover, this technology has also been applied to the pyrolysis of biomass and, in fact, a 25 kg h<sup>−</sup><sup>1</sup> pilot plant has been developed for this process [53, 54].

The main interest in analyzing the results obtained in the pyrolysis of the plastics lies in the fact that it constitutes the first step of the integrated pyrolysisreforming strategy, and therefore the volatile products of the pyrolysis process are the reactants of the catalytic reforming step. Consequently, it is essential to know the composition of the volatile stream leaving the pyrolysis step. Accordingly, the composition of the volatile stream for the pyrolysis of polyolefins (HDPE and PP), PET and PS, are analyzed in this section.

*Recent Advances in Pyrolysis*

The future of the hydrogen market is conditioned by the need to reduce CO2 emissions, which requires obtaining it from raw materials and renewable energy sources. The so-called hydrogen economy contemplates a future scenario in which this gas produced in a clean and economical way from a wide range of renewable sources would contribute to meeting the society's energy needs through combustion engines or preferably, by means of fuel cells, to a more efficient energy generation. This proposal would help to decentralize and diversify the energy system and

In this scenario, the processes aimed at hydrogen production from biomass and waste are gaining growing attention [1, 4–6], with the thermochemical routes being those with best perspectives for their full scale implementation. Thus, hydrogen production from waste plastics has been mainly approached by means of steam

Gasification allows for the conversion of waste plastics into a gaseous stream with varying contents of H2, CO, CO2, CH4 and N2 depending on process conditions and the gasifying agent used. The main advantage of gasification in relation to other thermochemical processes lies in its flexibility to valorize plastics of different composition or mixtures or plastics with other feedstocks. The main technologies for waste plastics gasification are those previously developed for biomass and coal gasification. It is to note that fluidized bed reactors have been widely used in the gasification of plastics [7–13]. However, these studies were mainly performed using air as fluidizing agent, so that the resulting gas has low hydrogen content and its main interest is restricted to energy production. The dual fluidized bed technology has been successfully applied to the steam gasification of plastics [13] and plastics mixtures with coal and biomass [14, 15]. The relevance of this technology is related with the fact that it allows overcoming the problems associated by the endothermic nature of the process. In spite of the promising results reported by Wilk et al. [13] in the gasification of different waste plastics, the high tar content in the syngas (above 100 g m<sup>−</sup><sup>3</sup>

challenge. However, waste plastic gasification has been scarcely studied in fixed bed reactors. Moreover, the results obtained are of preliminary nature as the reactors used are of laboratory scale and operate in batch regime [16–19]. Erkiaga et al. [20, 21] used the conical spouted bed reactor in the steam gasification of HDPE, and a hydrogen rich syngas was obtained with moderate tar contents. Moreover, this reactor design was also used subsequently in the co-gasification of HDPE and biomass (pine sawdust) with promising results [22]. The high temperatures attained in plasma reactors are also suitable for tar elimination, and this technology has therefore been

The hydrogen production from plastics via pyrolysis-reforming strategy has been recently proposed as an alternative to conventional gasification. The interest of this strategy lies in the fact that a tar free syngas is produced due to the high activity of the reforming catalyst. Moreover, the mild conditions in the reforming step and the physical separation of waste plastic impurities and the catalysts improve catalyst stability. Nevertheless, this strategy has been scarcely studied and the results reported were mainly obtained in lab scale units [6]. The studies by the team of Professor Williams [25–28] were carried out in a system in which pyrolysis is carried out in discontinuous regime in a fixed bed reactor and the volatiles are reformed in a second fixed bed. The reaction equipment used by the team of Professor Yoshikawa [29, 30] is a step forward, as it operates in continuous regime, although the use of fixed beds for pyrolysis and reforming can involve serious limitations for the process scale up. Czernik and French [31] made a step forward in this technology by studying the continuous pyrolysis and in-line reforming of polypropylene in a system of two in-line fluidized beds, with a commercial naphtha reforming catalyst. Erkiaga et al. [32] originally proposed a two-step reactor unit operating in continuous regime by

) is a great

reduce the current dependence on fossil fuels and air pollution [3].

gasification and pyrolysis-reforming processes [6].

proposed for the gasification of waste plastics [23, 24].

**70**

The different nature of the plastics studied led to volatile streams of different composition in their pyrolysis. It is to note that HDPE and PP are made up of saturated hydrocarbon chains, the thermal degradation of these chains mainly occurs by random radical scission mechanism, which gives way to a wide product distribution ranging from light gases to waxes. The fast pyrolysis conditions of the conical spouted bed reactor and especially the short residence time attained favor the selective formation of primary products, i.e., waxes and hydrocarbons in the diesel range, with the yield of gases, gasoline and aromatics being very low. However, in the PS chains aromatic rings are included, thus, the depolymerisation of this plastic leads to the formation of monomers (styrene), oligomers and other secondary products of aromatic nature. Due to the low temperature and the suitable features of the reactor used in this study, the product stream obtained in PS pyrolysis is mainly made up of styrene. Finally, PET is produced by polymerization of terephthalic acid and ethylene Glycerol. Accordingly, a wide product distribution with oxygenates and aromatics are formed in PET pyrolysis. The different nature of the pyrolysis product stream has a remarkable influence on its behavior in the reforming step, and the following section deals with this aspect.

According to the results obtained in previous studies, pyrolysis temperature was fixed at 500°C [47, 49, 52]. This temperature ensures a stable process without operational problems and minimizes secondary reactions of pyrolysis products and energy requirements. Moreover, below this temperature the plastic pyrolysis kinetic is very slow. Although the polymer degradation in the pyrolysis-reforming process occurs under steam atmosphere, the results obtained in previous studies using steam are very similar to those obtained using nitrogen as fluidizing agent, and therefore steam has hardly any effect at this temperature [33, 35]. This result is associated with the mild pyrolysis conditions used, 500°C, which hinders steam reactivity. The experiments were performed with continuous plastic feed and using a bed of inert sand in the pyrolysis of all the polymers studied.

The results obtained in the continuous pyrolysis of different plastics, HDPE, PP, PS and PET at 500°C are summarized in **Figure 1**. Due to the similar nature of HDPE and PP, similar product yields are obtained in their pyrolysis. As observed in **Figure 1**, the pyrolysis of polyolefins (HDPE and PP) leads to high yields of waxes (C21+) and liquid hydrocarbons in the diesel range (C12▬C20), with the yield of the gasoline fraction being low and that of gases below 1.5 wt%. It is to note that the solid residue formed in the pyrolysis of polyolefins is negligible, and therefore the whole product stream is fed into the fluidized bed for its reforming. Waxes are made up of long chain hydrocarbons and are solid at room temperature. However, these products do not cause any operational problem in the pyrolysis-reforming process as long as they are fully converted into gaseous products in the reforming step.

On the other hand, PET showed a wider product distribution that those observed in the case of polyolefins. A remarkable solid residue yield (7 wt%) was obtained in the pyrolysis of PET, with this residue being obtained coating the sand particles. The main product fraction in PET pyrolysis is the gaseous stream, whose yield is of 42.8 wt%. This gas is mainly made up of carbon monoxide and dioxide. In addition, a remarkable yield of a solid fraction (benzoic and benzoylformic acids) is obtained at room temperature, which accounts for 37.4 wt%. However, the yield of oil is the lowest (12.8 wt%) in the polymers studied.

The pyrolysis of PS leads to a high monomer recovery, with the yield of styrene being 70.6 wt%. The gaseous product yield is very low, 1.5 wt%, and that of the solid residue negligible. Thus, the product distribution obtained in PS pyrolysis is made up of styrene and other secondary products of aromatic nature.

**73**

implementation.

*conical spouted bed reactor at 500°C.*

**Figure 1.**

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

**3. Pyrolysis and in-line reforming of plastics**

these results as a consequence of the catalyst deactivation.

The fast pyrolysis of waste plastics has been extensively studied in the literature

Thus, the following section shows the results obtained in the reforming of HDPE derived pyrolysis volatiles carried out using the configuration described above, i.e., the conical spouted bed reactor for the pyrolysis step and the fluidized bed reactor for the catalytic steam reforming step. The aim of this research was to study how different operating conditions affect the reforming of HDPE pyrolysis volatiles. The parametric study includes the effect of temperature, space time and steam/plastic (S/P) ratio on the conversion, hydrogen production and the yields of the products both at zero time on stream and over time, taking into account the evolution of

[38, 55, 56], due to its interest for producing fuels and chemicals. Recently, the pyrolysis and in-line reforming route for hydrogen production has gained attention, with several studies published over the last years [30, 31, 57]. In this scenario, the optimization of the process operating conditions is essential for its industrial

*Product distributions obtained in the continuous pyrolysis of HDPE (a), PP (b), PET (c) and PS (d) in a* 

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

**Figure 1.**

*Recent Advances in Pyrolysis*

The different nature of the plastics studied led to volatile streams of different composition in their pyrolysis. It is to note that HDPE and PP are made up of saturated hydrocarbon chains, the thermal degradation of these chains mainly occurs by random radical scission mechanism, which gives way to a wide product distribution ranging from light gases to waxes. The fast pyrolysis conditions of the conical spouted bed reactor and especially the short residence time attained favor the selective formation of primary products, i.e., waxes and hydrocarbons in the diesel range, with the yield of gases, gasoline and aromatics being very low. However, in the PS chains aromatic rings are included, thus, the depolymerisation of this plastic leads to the formation of monomers (styrene), oligomers and other secondary products of aromatic nature. Due to the low temperature and the suitable features of the reactor used in this study, the product stream obtained in PS pyrolysis is mainly made up of styrene. Finally, PET is produced by polymerization of terephthalic acid and ethylene Glycerol. Accordingly, a wide product distribution with oxygenates and aromatics are formed in PET pyrolysis. The different nature of the pyrolysis product stream has a remarkable influence on its behavior in the

reforming step, and the following section deals with this aspect.

a bed of inert sand in the pyrolysis of all the polymers studied.

products in the reforming step.

oil is the lowest (12.8 wt%) in the polymers studied.

According to the results obtained in previous studies, pyrolysis temperature was fixed at 500°C [47, 49, 52]. This temperature ensures a stable process without operational problems and minimizes secondary reactions of pyrolysis products and energy requirements. Moreover, below this temperature the plastic pyrolysis kinetic is very slow. Although the polymer degradation in the pyrolysis-reforming process occurs under steam atmosphere, the results obtained in previous studies using steam are very similar to those obtained using nitrogen as fluidizing agent, and therefore steam has hardly any effect at this temperature [33, 35]. This result is associated with the mild pyrolysis conditions used, 500°C, which hinders steam reactivity. The experiments were performed with continuous plastic feed and using

The results obtained in the continuous pyrolysis of different plastics, HDPE, PP, PS and PET at 500°C are summarized in **Figure 1**. Due to the similar nature of HDPE and PP, similar product yields are obtained in their pyrolysis. As observed in **Figure 1**, the pyrolysis of polyolefins (HDPE and PP) leads to high yields of waxes (C21+) and liquid hydrocarbons in the diesel range (C12▬C20), with the yield of the gasoline fraction being low and that of gases below 1.5 wt%. It is to note that the solid residue formed in the pyrolysis of polyolefins is negligible, and therefore the whole product stream is fed into the fluidized bed for its reforming. Waxes are made up of long chain hydrocarbons and are solid at room temperature. However, these products do not cause any operational problem in the pyrolysis-reforming process as long as they are fully converted into gaseous

On the other hand, PET showed a wider product distribution that those observed in the case of polyolefins. A remarkable solid residue yield (7 wt%) was obtained in the pyrolysis of PET, with this residue being obtained coating the sand particles. The main product fraction in PET pyrolysis is the gaseous stream, whose yield is of 42.8 wt%. This gas is mainly made up of carbon monoxide and dioxide. In addition, a remarkable yield of a solid fraction (benzoic and benzoylformic acids) is obtained at room temperature, which accounts for 37.4 wt%. However, the yield of

The pyrolysis of PS leads to a high monomer recovery, with the yield of styrene being 70.6 wt%. The gaseous product yield is very low, 1.5 wt%, and that of the solid residue negligible. Thus, the product distribution obtained in PS pyrolysis is

made up of styrene and other secondary products of aromatic nature.

**72**

*Product distributions obtained in the continuous pyrolysis of HDPE (a), PP (b), PET (c) and PS (d) in a conical spouted bed reactor at 500°C.*

## **3. Pyrolysis and in-line reforming of plastics**

The fast pyrolysis of waste plastics has been extensively studied in the literature [38, 55, 56], due to its interest for producing fuels and chemicals. Recently, the pyrolysis and in-line reforming route for hydrogen production has gained attention, with several studies published over the last years [30, 31, 57]. In this scenario, the optimization of the process operating conditions is essential for its industrial implementation.

Thus, the following section shows the results obtained in the reforming of HDPE derived pyrolysis volatiles carried out using the configuration described above, i.e., the conical spouted bed reactor for the pyrolysis step and the fluidized bed reactor for the catalytic steam reforming step. The aim of this research was to study how different operating conditions affect the reforming of HDPE pyrolysis volatiles. The parametric study includes the effect of temperature, space time and steam/plastic (S/P) ratio on the conversion, hydrogen production and the yields of the products both at zero time on stream and over time, taking into account the evolution of these results as a consequence of the catalyst deactivation.

#### **3.1 Parametric study of HDPE pyrolysis and in-line reforming**

The results obtained in the parametric study carried out at zero time on stream are described below.

#### *3.1.1 Effect of temperature*

This section deals with the effect the reforming temperature in the 600–700°C range has on conversion, hydrogen production and gaseous products yields at zero time on stream. The operating conditions selected to carry out this study have been the following: (i) temperature in the pyrolysis step has been 500°C; (ii) a high space time of 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> (corresponding to 12.5 g of catalyst); (iii) steam/ plastic (S/P) ratio of 4. These conditions have been established in order to avoid operational problems. The space time value has been given as the amount of catalyst used by mass unit of the plastic fed into the pyrolysis reactor. High value of space time (16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> ) has been used in order to ensure high initial conversion of the volatiles coming from pyrolysis step and ensure a slow deactivation of the catalyst. Moreover, using a S/P ratio of 4 catalyst stability is guaranteed, given that coke gasification is favored and at the same time hydrogen production is increased.

The gaseous products quantified are as follows: H2, CO2, CO, CH4 and light hydrocarbon fraction (C2▬C4), composed mainly of ethylene, ethane, propylene and propane. The unreformed liquid fraction in the volatile stream coming from pyrolysis step has been called C5+ fraction. This fraction is conventionally called tar and should be removed in order for the product gas to be used as synthesis gas or conduct a further separation to isolate hydrogen.

The evolution of the conversion and hydrogen production with temperature is shown in **Figure 2a** and **b** shows the evolution of gaseous products yields with temperature. In order to quantify the results obtained in the reforming step, some reaction indices have been defined. The conversion is defined as the carbon conversion efficiency, i.e., the percentage of carbon moles contained in the plastic feed that are recovered in the gaseous products. **Figure 2a** shows that the conversion is greater than 94% in the temperature range studied. In addition, an increase in temperature enhances the reforming reaction, achieving a conversion of 98% at 700°C. Therefore, at this temperature only 2% of the carbon fed, which is in the C5+ fraction of the product stream, remains without transforming into gas. It should be noted that, at the temperature range studied, the conversion of hydrocarbons entering the reforming reactor (mostly waxes as aforementioned in the previous section) is almost full. This trend is characteristic of steam reforming reactions [29, 58], which is because the endothermic hydrocarbon reforming reactions and cracking reactions are enhanced as temperature is increased.

Another interesting index for quantify the results obtained is hydrogen production. This index is calculated as the mass of hydrogen produced per plastic mass unit fed into the pyrolysis step. **Figure 2a** shows the evolution of hydrogen production with temperature. The production of hydrogen increases with temperature, reaching a value of 37.3 wt% at 700°C. In fact, as temperature is increased the endothermic reaction of reforming is favored, enhancing hydrogen production. Based on the mass balance of hydrogen, approximately 63% of this hydrogen is formed from steam and the remaining 37% from the plastic. This hydrogen production is slightly higher than that obtained by Czernik and French [31], 34 wt%, in their study of pyrolysis-reforming of PP.

The increase in conversion and hydrogen production with temperature in the catalytic steam reforming of municipal solid wastes [59] is explained because all the endothermic steps involved are favored: (i) initial pyrolysis of waste; (ii) char

**75**

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

gasification reactions; (iii) cracking and steam reforming of the tar. In the latter case, the increase in temperature enhances the endothermic reactions of reforming,

*on product yields. Reaction conditions: Tpyrolysis, 500°C; space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>*

*(a) Evolution of HDPE conversion and hydrogen production with temperature; (b) effect of reforming temperature* 

 *and S/P ratio: 4.*

shift in the equilibrium of the water-gas shift (WGS) exothermic reaction. The increase in the yield of hydrogen and CO is because an increase in the reforming temperature favors the reforming of waxes, light hydrocarbons and CH4. Thus, although CH4, C2▬C4 and C5+ yields are very low in the whole temperature range studied, a slight decrease is observed as temperature is increased, obtaining yields of 0.8, 0.7 and 1.9% at 700°C, respectively. This result indicates the reforming of these compounds is enhanced selectively over their formation by cracking. On the other hand, it must be taken into account that the WGS reaction is exothermic, and therefore its thermodynamic equilibrium shift towards CO formation by

The effect the space time has on the reforming step has been studied in the

(i) temperature in the pyrolysis step, 500°C; (ii) temperature in the reforming step, 700°C; (iii) S/P ratio, 4. As in the previous section, the effect of space time on the conversion, hydrogen production and gaseous products yields has been studied. **Figure 3** shows the evolution with space time of conversion and hydrogen production (**Figure 3a**) and of the products yields (**Figure 3b**). As observed in **Figure 3a**,

range, by varying the amount of the catalyst, with the

. The remaining conditions are as follows:

**Figure 2b** shows the effect reforming temperature in the 600–700°C range has on products yields. Product yields are the reaction indices defined for the assessment of the reforming step performance. The yield of C containing individual compounds is defined by mass unit of plastic in the feed, and the hydrogen yield is a percentage of the maximum allowed by stoichiometry, which accounts for the hydrogen coming from the polymer and the steam. **Figure 2b** reveals that an increase in the reforming temperature leads to an increase in the yields of hydrogen, from 78.1% at 600°C to 85.7% at 700°C. Simultaneously, it is observed that temperature increase favors the formation of CO, obtaining a yield of 29.2% at 700°C. The effect of temperature on the CO2 yield is lower, since it remains constant due to the

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

as well as cracking.

**Figure 2.**

increasing temperature.

*3.1.2 Effect of space time*

2.8–20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

plastic feed rate being 0.75 g min<sup>−</sup><sup>1</sup>

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

**Figure 2.** *(a) Evolution of HDPE conversion and hydrogen production with temperature; (b) effect of reforming temperature on product yields. Reaction conditions: Tpyrolysis, 500°C; space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> and S/P ratio: 4.*

gasification reactions; (iii) cracking and steam reforming of the tar. In the latter case, the increase in temperature enhances the endothermic reactions of reforming, as well as cracking.

**Figure 2b** shows the effect reforming temperature in the 600–700°C range has on products yields. Product yields are the reaction indices defined for the assessment of the reforming step performance. The yield of C containing individual compounds is defined by mass unit of plastic in the feed, and the hydrogen yield is a percentage of the maximum allowed by stoichiometry, which accounts for the hydrogen coming from the polymer and the steam. **Figure 2b** reveals that an increase in the reforming temperature leads to an increase in the yields of hydrogen, from 78.1% at 600°C to 85.7% at 700°C. Simultaneously, it is observed that temperature increase favors the formation of CO, obtaining a yield of 29.2% at 700°C. The effect of temperature on the CO2 yield is lower, since it remains constant due to the shift in the equilibrium of the water-gas shift (WGS) exothermic reaction.

The increase in the yield of hydrogen and CO is because an increase in the reforming temperature favors the reforming of waxes, light hydrocarbons and CH4. Thus, although CH4, C2▬C4 and C5+ yields are very low in the whole temperature range studied, a slight decrease is observed as temperature is increased, obtaining yields of 0.8, 0.7 and 1.9% at 700°C, respectively. This result indicates the reforming of these compounds is enhanced selectively over their formation by cracking. On the other hand, it must be taken into account that the WGS reaction is exothermic, and therefore its thermodynamic equilibrium shift towards CO formation by increasing temperature.

#### *3.1.2 Effect of space time*

The effect the space time has on the reforming step has been studied in the 2.8–20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> range, by varying the amount of the catalyst, with the plastic feed rate being 0.75 g min<sup>−</sup><sup>1</sup> . The remaining conditions are as follows: (i) temperature in the pyrolysis step, 500°C; (ii) temperature in the reforming step, 700°C; (iii) S/P ratio, 4. As in the previous section, the effect of space time on the conversion, hydrogen production and gaseous products yields has been studied.

**Figure 3** shows the evolution with space time of conversion and hydrogen production (**Figure 3a**) and of the products yields (**Figure 3b**). As observed in **Figure 3a**,

*Recent Advances in Pyrolysis*

are described below.

*3.1.1 Effect of temperature*

time of 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

time (16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

conduct a further separation to isolate hydrogen.

reactions are enhanced as temperature is increased.

**3.1 Parametric study of HDPE pyrolysis and in-line reforming**

The results obtained in the parametric study carried out at zero time on stream

This section deals with the effect the reforming temperature in the 600–700°C range has on conversion, hydrogen production and gaseous products yields at zero time on stream. The operating conditions selected to carry out this study have been the following: (i) temperature in the pyrolysis step has been 500°C; (ii) a high space

plastic (S/P) ratio of 4. These conditions have been established in order to avoid operational problems. The space time value has been given as the amount of catalyst used by mass unit of the plastic fed into the pyrolysis reactor. High value of space

sion of the volatiles coming from pyrolysis step and ensure a slow deactivation of the catalyst. Moreover, using a S/P ratio of 4 catalyst stability is guaranteed, given that coke gasification is favored and at the same time hydrogen production is increased. The gaseous products quantified are as follows: H2, CO2, CO, CH4 and light hydrocarbon fraction (C2▬C4), composed mainly of ethylene, ethane, propylene and propane. The unreformed liquid fraction in the volatile stream coming from pyrolysis step has been called C5+ fraction. This fraction is conventionally called tar and should be removed in order for the product gas to be used as synthesis gas or

The evolution of the conversion and hydrogen production with temperature is shown in **Figure 2a** and **b** shows the evolution of gaseous products yields with temperature. In order to quantify the results obtained in the reforming step, some reaction indices have been defined. The conversion is defined as the carbon conversion efficiency, i.e., the percentage of carbon moles contained in the plastic feed that are recovered in the gaseous products. **Figure 2a** shows that the conversion is greater than 94% in the temperature range studied. In addition, an increase in temperature enhances the reforming reaction, achieving a conversion of 98% at 700°C. Therefore, at this temperature only 2% of the carbon fed, which is in the C5+ fraction of the product stream, remains without transforming into gas. It should be noted that, at the temperature range studied, the conversion of hydrocarbons entering the reforming reactor (mostly waxes as aforementioned in the previous section) is almost full. This trend is characteristic of steam reforming reactions [29, 58], which is because the endothermic hydrocarbon reforming reactions and cracking

Another interesting index for quantify the results obtained is hydrogen production. This index is calculated as the mass of hydrogen produced per plastic mass unit fed into the pyrolysis step. **Figure 2a** shows the evolution of hydrogen production with temperature. The production of hydrogen increases with temperature, reaching a value of 37.3 wt% at 700°C. In fact, as temperature is increased the endothermic reaction of reforming is favored, enhancing hydrogen production. Based on the mass balance of hydrogen, approximately 63% of this hydrogen is formed from steam and the remaining 37% from the plastic. This hydrogen production is slightly higher than that obtained by Czernik and French [31], 34 wt%, in their study of

The increase in conversion and hydrogen production with temperature in the catalytic steam reforming of municipal solid wastes [59] is explained because all the endothermic steps involved are favored: (i) initial pyrolysis of waste; (ii) char

(corresponding to 12.5 g of catalyst); (iii) steam/

) has been used in order to ensure high initial conver-

**74**

pyrolysis-reforming of PP.

**Figure 3.**

*(a) Evolution of HDPE conversion and hydrogen production with space time; (b) effect of space time on product yields. Reaction conditions: Tpyrolysis, 500°C; Treforming, 700°C; and S/P ratio, 4.*

there is a sharp increase in conversion when space time is increased from 2.8 (68.3%) to 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> (97.5%). An increase in space time above the latter value only contributes to slightly increasing conversion, which is almost full (99.7%) for a space time of 20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> . Regarding hydrogen production, it increases from 18.6 wt% at 2.8 to 38 wt% at 20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> . The production of hydrogen increases more significantly in the space time range from 2.8 to 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> , whereas in the 8.3–20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> range the increase is milder.

**Figure 3b** shows the effect space time in the 2.8–20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> range has on product yields. By enhancing the extent of reforming reactions and WGS reactions, the increase in space time increases the yields of hydrogen, CO2 and CO, whereas it decreases the yields of CH4, C2▬C4 and C5+. An increase in space time (**Figure 3a**) from 2.8 to 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> leads to a pronounced increase in the yield of hydrogen and CO2 to 73.8 and 69.3%, respectively. In the mentioned range of space time, the increase in CO yield is less significant, reaching a value of 23.2% for 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> . Therefore, it seems that increasing space time in this range the WGS reaction is selectively favored. It is also important to highlight the decrease in the yields of CH4, C2▬C4 and C5+, especially in the case of C2▬C4 and C5+, whose yields decrease from 27.2 to 3.8%, and from 31.7 to 2.4%, respectively, in the 2.8–8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> range.

For space times higher than 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> there is hardly any change in the yields. However, in the case of hydrogen, its yield continues increasing, reaching 86.7% for a space time of 20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> . On the other hand, an increase in space time from 8.3 to 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> hardly affects CO2 yield, whereas it leads to a slight decrease in CO, which reaches a maximum value of 29.3%.

The remarkable effect of space time on conversion and gaseous product yields is well established in the literature in both the pyrolysis and reforming of plastics [60] and the gasification and reforming of municipal solid waste [59, 61, 62], which is explained by the enhancement of the reforming and WGS reactions.

#### *3.1.3 Effect of steam/plastic (S/P) ratio*

In this section, the effect S/P ratio in the 3–5 range has on conversion, hydrogen production and products yields at zero time on stream is shown. The operating conditions selected to carry out this study have been the following: (i) temperature

**77**

**Figure 4.**

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

of the pyrolysis step, 500°C; (ii) temperature of the reforming step, 700°C;

the steam partial pressure, thus the steam partial pressure in the reaction medium is

**Figure 4** shows the evolution of conversion and hydrogen production with the steam/plastic (S/P) ratio (**Figure 4a**), as well as the evolution of products yields with S/P ratio (**Figure 4b**). **Figure 4a** shows that in the S/P range studied conversion is over 98%, reaching almost 99.6% with a ratio of 5. By increasing the S/P ratio from 3 to 4, the effect of the ratio is not very relevant and, as mentioned above, by increasing to 5 conversion is almost full. The reaction rate of the reforming and WGS reactions are enhanced by increasing the steam partial pressure in the reaction environment, which explains the high conversions obtained. Consequently, hydrogen production significantly increases in the S/P range studied, from 31.0 wt% for a

**Figure 4b** displays the effect S/P ratio in the 3–5 range has on product yields. It is observed that an increase in this ratio leads to a progressive increase in the hydrogen and CO2 yields and a decrease in those of CO, CH4, C2▬C4 and C5+. This effect is due to the higher concentration of steam in the reaction environment, which favors the displacement of both hydrocarbons reforming reactions and the WGS reaction. By favoring all the reactions involved in the reforming, an increase in the S/P ratio enhances the yield of hydrogen and CO2, up to 92.5 and 80.9% for a ratio of 5. Consequently, the yield of CO decreases to 18.1%. The yields of CH4, C2▬C4 and C5+, which are small for a S/P ratio of 4, decrease until becoming insignificant. As observed, an increase in S/P ratio causes a positive effect on conversion and hydrogen production; however, an excessive increase affects significantly on the

Qualitatively similar effects of S/P ratio were observed in the pyrolysis-reforming of PP [63, 64], LDPE and PS [63] and municipal plastic wastes [65], which is a widely proven fact in the gasification of different polymeric materials [58, 66].

Knowledge of catalyst deactivation is essential for its choice, design of the reactor and establishment of the optimal strategy for the operation of industrial

*(a) Evolution of HDPE conversion and hydrogen production with S/P ratio; (b) effect of the S/P ratio on product yields. Reaction conditions: Tpyrolysis, 500°C; Treforming, 700°C; and space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>*

*.*

. The effect of S/P ratio is directly related to

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

(iii) space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

more significant when this ratio is increased.

S/P ratio of 3 to 38.1 wt% for a S/P ratio of 5.

energy efficiency of the process.

*3.1.4 Catalyst deactivation*

#### *Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

of the pyrolysis step, 500°C; (ii) temperature of the reforming step, 700°C; (iii) space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> . The effect of S/P ratio is directly related to the steam partial pressure, thus the steam partial pressure in the reaction medium is more significant when this ratio is increased.

**Figure 4** shows the evolution of conversion and hydrogen production with the steam/plastic (S/P) ratio (**Figure 4a**), as well as the evolution of products yields with S/P ratio (**Figure 4b**). **Figure 4a** shows that in the S/P range studied conversion is over 98%, reaching almost 99.6% with a ratio of 5. By increasing the S/P ratio from 3 to 4, the effect of the ratio is not very relevant and, as mentioned above, by increasing to 5 conversion is almost full. The reaction rate of the reforming and WGS reactions are enhanced by increasing the steam partial pressure in the reaction environment, which explains the high conversions obtained. Consequently, hydrogen production significantly increases in the S/P range studied, from 31.0 wt% for a S/P ratio of 3 to 38.1 wt% for a S/P ratio of 5.

**Figure 4b** displays the effect S/P ratio in the 3–5 range has on product yields. It is observed that an increase in this ratio leads to a progressive increase in the hydrogen and CO2 yields and a decrease in those of CO, CH4, C2▬C4 and C5+. This effect is due to the higher concentration of steam in the reaction environment, which favors the displacement of both hydrocarbons reforming reactions and the WGS reaction. By favoring all the reactions involved in the reforming, an increase in the S/P ratio enhances the yield of hydrogen and CO2, up to 92.5 and 80.9% for a ratio of 5. Consequently, the yield of CO decreases to 18.1%. The yields of CH4, C2▬C4 and C5+, which are small for a S/P ratio of 4, decrease until becoming insignificant.

As observed, an increase in S/P ratio causes a positive effect on conversion and hydrogen production; however, an excessive increase affects significantly on the energy efficiency of the process.

Qualitatively similar effects of S/P ratio were observed in the pyrolysis-reforming of PP [63, 64], LDPE and PS [63] and municipal plastic wastes [65], which is a widely proven fact in the gasification of different polymeric materials [58, 66].

#### *3.1.4 Catalyst deactivation*

*Recent Advances in Pyrolysis*

to 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

**Figure 3.**

for 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

the 2.8–8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

time of 20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

18.6 wt% at 2.8 to 38 wt% at 20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

whereas in the 8.3–20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

(**Figure 3a**) from 2.8 to 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

there is a sharp increase in conversion when space time is increased from 2.8 (68.3%)

*(a) Evolution of HDPE conversion and hydrogen production with space time; (b) effect of space time on* 

*product yields. Reaction conditions: Tpyrolysis, 500°C; Treforming, 700°C; and S/P ratio, 4.*

contributes to slightly increasing conversion, which is almost full (99.7%) for a space

increases more significantly in the space time range from 2.8 to 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

**Figure 3b** shows the effect space time in the 2.8–20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

has on product yields. By enhancing the extent of reforming reactions and WGS reactions, the increase in space time increases the yields of hydrogen, CO2 and CO, whereas it decreases the yields of CH4, C2▬C4 and C5+. An increase in space time

yield of hydrogen and CO2 to 73.8 and 69.3%, respectively. In the mentioned range of space time, the increase in CO yield is less significant, reaching a value of 23.2%

range the WGS reaction is selectively favored. It is also important to highlight the decrease in the yields of CH4, C2▬C4 and C5+, especially in the case of C2▬C4 and C5+, whose yields decrease from 27.2 to 3.8%, and from 31.7 to 2.4%, respectively, in

the yields. However, in the case of hydrogen, its yield continues increasing, reaching

The remarkable effect of space time on conversion and gaseous product yields is well established in the literature in both the pyrolysis and reforming of plastics [60] and the gasification and reforming of municipal solid waste [59, 61, 62], which is

In this section, the effect S/P ratio in the 3–5 range has on conversion, hydrogen production and products yields at zero time on stream is shown. The operating conditions selected to carry out this study have been the following: (i) temperature

range.

leads to a slight decrease in CO, which reaches a maximum value of 29.3%.

explained by the enhancement of the reforming and WGS reactions.

For space times higher than 8.3 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

86.7% for a space time of 20.8 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

space time from 8.3 to 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

*3.1.3 Effect of steam/plastic (S/P) ratio*

(97.5%). An increase in space time above the latter value only

. Regarding hydrogen production, it increases from

range the increase is milder.

. Therefore, it seems that increasing space time in this

. The production of hydrogen

leads to a pronounced increase in the

there is hardly any change in

. On the other hand, an increase in

hardly affects CO2 yield, whereas it

,

range

**76**

Knowledge of catalyst deactivation is essential for its choice, design of the reactor and establishment of the optimal strategy for the operation of industrial

**Figure 4.**

*(a) Evolution of HDPE conversion and hydrogen production with S/P ratio; (b) effect of the S/P ratio on product yields. Reaction conditions: Tpyrolysis, 500°C; Treforming, 700°C; and space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> .*

catalytic processes. It is well documented that coke deposition is the main cause of catalyst deactivation in the pyrolysis-reforming of plastics [63, 67], as well as in the reforming of hydrocarbons and oxygenates (methanol, DME, ethanol, bio-oil) [68, 69]. This deposition is especially important for Ni based catalysts.

The commercial catalyst used in this study does not undergo a significant Ni sintering because it is designed to use in CH4 reforming, which is a reaction carried out at a temperature of around 850°C, i.e., higher than the highest used in this study (700°C). The plastics used do not contain S, and therefore the deactivation cause is the deposition of coke. Three different types of coke have been identified in the reforming of CH4 on Ni catalyst: pyrolytic, encapsulating and filamentous [70]. Numerous studies support this classification of the coke deposited in the reforming of CH4, hydrocarbons and biomass derivates.

Wu and Williams [26] have verified by transmission electron microscopy (TEM) that the coke deposited on Ni catalyst used in the production of hydrogen by pyrolysis-reforming of PP is composed of two types of coke, amorphous and filamentous, with the latter having similar characteristics as carbon nanotubes and graphene (according to their graphitization degree). Considering the commercial interest of filamentous coke for these applications, Acomb et al. [63] have studied the simultaneous production of carbon nanotubes and hydrogen through pyrolysisreforming of PP, which improves the economy of the process and provides an additional incentive for the viability of plastic recycling.

In this section, a study is carried out of the effect catalyst deactivation has on conversion and product yields with time on stream. The reaction conditions used are as follows: (i) temperature in the pyrolysis step, 500°C; (ii) temperature in the reforming step, 700°C; (iii) space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> and (iv) S/P ratio, 4. The study has been carried out under conditions in which a slow deactivation of the catalyst is observed, evaluating the effect of the incipient deposition of coke and the evolution of this deposition up to 123 min of reaction.

**Figure 5** shows the effect catalyst deactivation has on plastics conversion (**Figure 5a**) and product yields (**Figure 5b**). As observed, whilst the reforming reaction progresses with time on stream the conversion of plastics decreases due to the deactivation undergone by the catalyst, decreasing linearly from 98.1% at zero time on stream to 90.3% in 123 min. Besides, comparing the evolution of conversion (**Figure 5a**) and the evolution of product yields (**Figure 5b**), the decrease in H2 and CO2 yields decrease in a similar trend to that of conversion, as catalyst deactivation hinders the reforming reaction, as well as the WGS reaction. Consequently, CH4, C2▬C4 and C5+ hydrocarbon yields increase. As observed in **Figure 5**, the conversion and the yields of H2 and CO2 decrease linearly and those of CH4, C2▬C4 and C5+ hydrocarbons increase linearly. The lineal catalyst deactivation rate observed should be attributed to: (i) high temperature favoring the kinetics of reforming reactions due to their endothermic nature, which leads to a low concentration of hydrocarbons in the reaction medium, and therefore low coke deposition rate (low catalyst deactivation); (ii) high temperature enhances the gasification of the deposited coke and so minimize catalyst deactivation [68].

As a result of reforming activity decrease, CH4, C2▬C4 and C5+ fraction yields increase over time, which is more noticeable as the molecular weight of the hydrocarbons increases. This trend is explained by the reforming of C5+ hydrocarbons in parallel with the thermal cracking of these compounds towards CH4 and C2▬C4. Consequently, as reforming rate decreases due to catalyst deactivation the thermal cracking reactions are favored. This cracking phenomenon is well known in deactivated catalysts and is more important as the molecular weight of aliphatic compounds is higher [71].

**79**

**Figure 6.**

*TPO profile of the coke deposited on the catalyst.*

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

formation of ethylene and benzene, is higher than that of paraffin compounds [71]. It is also well recognized that the coke formed on a Ni catalyst at high temperature is

*(a) Evolution of HDPE conversion with time on stream; (b) evolution of product yields with time on stream.* 

**Figure 6** displays a temperature programmed oxidation (TPO) profile of the coke deposited on the catalyst after 123 min reaction. Moreover, an average coke deposition rate has been quantified in order to calculate the extent of coke deposition. According to the TPO profile obtained, it has been determined that the average

peaks may be observed in **Figure 6**, which are evidence of two cokes of different

gHDPE<sup>−</sup><sup>1</sup>

. Furthermore, two different

*; S/P = 4.*

more filamentous and with less capacity for blocking Ni sites [68, 71].

*Reaction conditions: Tpyrolysis, 500°C; Treforming, 700°C; space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>*

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

coke deposition rate is 0.7 mgcoke gcatalyst<sup>−</sup><sup>1</sup>

**Figure 5.**

It is established in the literature that paraffin capacity for coke formation is greater as their molecular weight is higher [72]. Similarly, the capacity for coke *Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

#### **Figure 5.**

*Recent Advances in Pyrolysis*

catalytic processes. It is well documented that coke deposition is the main cause of catalyst deactivation in the pyrolysis-reforming of plastics [63, 67], as well as in the reforming of hydrocarbons and oxygenates (methanol, DME, ethanol, bio-oil) [68, 69].

The commercial catalyst used in this study does not undergo a significant Ni sintering because it is designed to use in CH4 reforming, which is a reaction carried out at a temperature of around 850°C, i.e., higher than the highest used in this study (700°C). The plastics used do not contain S, and therefore the deactivation cause is the deposition of coke. Three different types of coke have been identified in the reforming of CH4 on Ni catalyst: pyrolytic, encapsulating and filamentous [70]. Numerous studies support this classification of the coke deposited in the reforming

Wu and Williams [26] have verified by transmission electron microscopy (TEM) that the coke deposited on Ni catalyst used in the production of hydrogen by pyrolysis-reforming of PP is composed of two types of coke, amorphous and filamentous, with the latter having similar characteristics as carbon nanotubes and graphene (according to their graphitization degree). Considering the commercial interest of filamentous coke for these applications, Acomb et al. [63] have studied the simultaneous production of carbon nanotubes and hydrogen through pyrolysisreforming of PP, which improves the economy of the process and provides an

In this section, a study is carried out of the effect catalyst deactivation has on conversion and product yields with time on stream. The reaction conditions used are as follows: (i) temperature in the pyrolysis step, 500°C; (ii) temperature in the

The study has been carried out under conditions in which a slow deactivation of the catalyst is observed, evaluating the effect of the incipient deposition of coke and the

**Figure 5** shows the effect catalyst deactivation has on plastics conversion (**Figure 5a**) and product yields (**Figure 5b**). As observed, whilst the reforming reaction progresses with time on stream the conversion of plastics decreases due to the deactivation undergone by the catalyst, decreasing linearly from 98.1% at zero time on stream to 90.3% in 123 min. Besides, comparing the evolution of conversion (**Figure 5a**) and the evolution of product yields (**Figure 5b**), the decrease in H2 and CO2 yields decrease in a similar trend to that of conversion, as catalyst deactivation hinders the reforming reaction, as well as the WGS reaction. Consequently, CH4, C2▬C4 and C5+ hydrocarbon yields increase. As observed in **Figure 5**, the conversion and the yields of H2 and CO2 decrease linearly and those of CH4, C2▬C4 and C5+ hydrocarbons increase linearly. The lineal catalyst deactivation rate observed should be attributed to: (i) high temperature favoring the kinetics of reforming reactions due to their endothermic nature, which leads to a low concentration of hydrocarbons in the reaction medium, and therefore low coke deposition rate (low catalyst deactivation); (ii) high temperature enhances the gasification of the

As a result of reforming activity decrease, CH4, C2▬C4 and C5+ fraction yields increase over time, which is more noticeable as the molecular weight of the hydrocarbons increases. This trend is explained by the reforming of C5+ hydrocarbons in parallel with the thermal cracking of these compounds towards CH4 and C2▬C4. Consequently, as reforming rate decreases due to catalyst deactivation the thermal cracking reactions are favored. This cracking phenomenon is well known in deactivated catalysts and is more important as the molecular weight of aliphatic compounds is higher [71]. It is established in the literature that paraffin capacity for coke formation is greater as their molecular weight is higher [72]. Similarly, the capacity for coke

and (iv) S/P ratio, 4.

This deposition is especially important for Ni based catalysts.

of CH4, hydrocarbons and biomass derivates.

additional incentive for the viability of plastic recycling.

evolution of this deposition up to 123 min of reaction.

deposited coke and so minimize catalyst deactivation [68].

reforming step, 700°C; (iii) space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

**78**

*(a) Evolution of HDPE conversion with time on stream; (b) evolution of product yields with time on stream. Reaction conditions: Tpyrolysis, 500°C; Treforming, 700°C; space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> ; S/P = 4.*

formation of ethylene and benzene, is higher than that of paraffin compounds [71]. It is also well recognized that the coke formed on a Ni catalyst at high temperature is more filamentous and with less capacity for blocking Ni sites [68, 71].

**Figure 6** displays a temperature programmed oxidation (TPO) profile of the coke deposited on the catalyst after 123 min reaction. Moreover, an average coke deposition rate has been quantified in order to calculate the extent of coke deposition. According to the TPO profile obtained, it has been determined that the average coke deposition rate is 0.7 mgcoke gcatalyst<sup>−</sup><sup>1</sup> gHDPE<sup>−</sup><sup>1</sup> . Furthermore, two different peaks may be observed in **Figure 6**, which are evidence of two cokes of different

**Figure 6.** *TPO profile of the coke deposited on the catalyst.*

nature and location on the catalyst. The main peak appears at 550°C and accounts for a partially structured coke, whereas the second peak at 430°C corresponds to an encapsulating coke, which is deposited on the Ni metal.

The encapsulating coke is deposited close to the actives sites, which promote coke combustion. Furthermore, this amorphous structure hinders the adsorption of reactants, which increases the concentration of non-converted hydrocarbons in the reaction environment, and consequently deactivates the catalyst. On the other hand, the combustion of the partially structured coke occurs at higher temperature due to the further location of the coke from the metallic sites, thereby hindering its combustion [63, 73]. This type of deposited coke corresponds to the filamentous coke, which generally does not affect directly to catalyst deactivation, as it does not block the active sites [69]. However, when its content is severe, it blocks the active sites, hindering the adsorption of reactants, and consequently increasing the concentration of non-converted hydrocarbons in the reaction medium.

The aforementioned identification of two types of coke has been corroborated based on the scanning electron microscopy (SEM) image of the deactivated catalyst displayed in **Figure 7**. It should be noted that the nature of the coke deposited on the deactivated catalyst at 123 min reaction is amorphous and fibrillary. Ochoa et al. [74] demonstrated that coke content evolves with time on stream. In this evolution, both types of cokes growth throughout time on stream with different rates, with the one for filamentous coke being higher. However, it can be concluded that coke deposition is more influenced by the growth of encapsulating coke, as has also been established in the literature [75, 76].

## **3.2 Pyrolysis and in-line reforming of different plastics**

Approximately 40% of the post-consumption wastes come from agriculture, construction, automotive and distribution sectors, and the remaining 60% from municipal solid wastes (MSW). Although the plastics only account for 7 wt% in the MSW, its contribution is 20 vol% of the total MSW volume. Therefore, the

**81**

**Figure 8.**

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

thermochemical routes are of especial relevance for plastic valorization for obtaining fuels or for the production of chemical products, such as hydrogen. Moreover, the large scale viability of these processes will presumably require the joint valorization of different plastics from MSW. Accordingly, this section deals with the valorization of plastics of different nature by means of pyrolysis and in-line reforming strategy in order to evaluate its feasibility. Based on their production scale, the following plastics were selected: high density polyethylene (HDPE), polypropylene (PP), polyethylene terephthalate (PET) and polystyrene (PS). The operating conditions selected to carry out this study have been as follows: (i) temperature of the pyrolysis step, 500°C; (ii) temperature of the reforming step, 700°C; (iii) space

; (iv) S/P ratio of 4. The hydrogen produced in the pyrolysis and in-line catalytic reforming of different plastics is shown in **Figure 8a**. As observed, the highest hydrogen production is obtained when HDPE and PP are used as feed, 37.3 and 34.8 wt%, respectively, followed by PS (29.1 wt%), which has a lower hydrogen content in its composition. However, the oxygenated nature of the PET and the residue formed in its pyrolysis step leads to a lower hydrogen production in the reforming step (18.2 wt%). Wu and Williams [26] also observed lower conversion of PS pyrolysis volatiles compared to HDPE in the pyrolysis and in-line reforming of different plastics. A hydrogen production of 34 wt% was obtained by Czernik and French [31] in the pyrolysis and in-line reforming of PP using two fluidized bed reactors. Namioka et al. [29] performed the pyrolysis-reforming of PP and PS, with hydrogen production being 36 and 33 wt%, respectively. Recently, Saad and Williams [28] studied the pyrolysis and in-line dry reforming of different plastics, obtaining hydrogen productions of

It should be highlighted that the Ni catalyst used for the pyrolysis-reforming process allows achieving a high conversion of pyrolysis products to gases (>98%),

obtained in the literature on Ru catalysts. Park et al. [30] obtained a similar conversion in the pyrolysis-reforming of PP, in a continuous regime system consisting of fixed bed reactors at 400 and 630°C, respectively, and using a space time of

of using Ru catalysts instead of Ni is the reduction of the reforming temperature by 70°C. Namioka et al. [29] extended the study using Ru catalysts to the pyrolysisreforming of PS, verifying that under the indicated conditions the differences

*Hydrogen production (a) and product yields (b) in the pyrolysis and in-line reforming of different plastics.*

. This result is comparable to those

. Based on this result, these authors note that the advantage

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

15, 7.6 and 2.5 wt% for PE, PS and PET, respectively.

with a space time of 16.7 gcatalyst min gplastic<sup>−</sup><sup>1</sup>

9.8 gcatalyst min gplastic<sup>−</sup><sup>1</sup>

**Figure 7.** *SEM image of the deactivated catalyst.*

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

thermochemical routes are of especial relevance for plastic valorization for obtaining fuels or for the production of chemical products, such as hydrogen. Moreover, the large scale viability of these processes will presumably require the joint valorization of different plastics from MSW. Accordingly, this section deals with the valorization of plastics of different nature by means of pyrolysis and in-line reforming strategy in order to evaluate its feasibility. Based on their production scale, the following plastics were selected: high density polyethylene (HDPE), polypropylene (PP), polyethylene terephthalate (PET) and polystyrene (PS). The operating conditions selected to carry out this study have been as follows: (i) temperature of the pyrolysis step, 500°C; (ii) temperature of the reforming step, 700°C; (iii) space time, 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> ; (iv) S/P ratio of 4.

The hydrogen produced in the pyrolysis and in-line catalytic reforming of different plastics is shown in **Figure 8a**. As observed, the highest hydrogen production is obtained when HDPE and PP are used as feed, 37.3 and 34.8 wt%, respectively, followed by PS (29.1 wt%), which has a lower hydrogen content in its composition. However, the oxygenated nature of the PET and the residue formed in its pyrolysis step leads to a lower hydrogen production in the reforming step (18.2 wt%). Wu and Williams [26] also observed lower conversion of PS pyrolysis volatiles compared to HDPE in the pyrolysis and in-line reforming of different plastics. A hydrogen production of 34 wt% was obtained by Czernik and French [31] in the pyrolysis and in-line reforming of PP using two fluidized bed reactors. Namioka et al. [29] performed the pyrolysis-reforming of PP and PS, with hydrogen production being 36 and 33 wt%, respectively. Recently, Saad and Williams [28] studied the pyrolysis and in-line dry reforming of different plastics, obtaining hydrogen productions of 15, 7.6 and 2.5 wt% for PE, PS and PET, respectively.

It should be highlighted that the Ni catalyst used for the pyrolysis-reforming process allows achieving a high conversion of pyrolysis products to gases (>98%), with a space time of 16.7 gcatalyst min gplastic<sup>−</sup><sup>1</sup> . This result is comparable to those obtained in the literature on Ru catalysts. Park et al. [30] obtained a similar conversion in the pyrolysis-reforming of PP, in a continuous regime system consisting of fixed bed reactors at 400 and 630°C, respectively, and using a space time of 9.8 gcatalyst min gplastic<sup>−</sup><sup>1</sup> . Based on this result, these authors note that the advantage of using Ru catalysts instead of Ni is the reduction of the reforming temperature by 70°C. Namioka et al. [29] extended the study using Ru catalysts to the pyrolysisreforming of PS, verifying that under the indicated conditions the differences

**Figure 8.** *Hydrogen production (a) and product yields (b) in the pyrolysis and in-line reforming of different plastics.*

*Recent Advances in Pyrolysis*

established in the literature [75, 76].

**3.2 Pyrolysis and in-line reforming of different plastics**

nature and location on the catalyst. The main peak appears at 550°C and accounts for a partially structured coke, whereas the second peak at 430°C corresponds to an

The encapsulating coke is deposited close to the actives sites, which promote coke combustion. Furthermore, this amorphous structure hinders the adsorption of reactants, which increases the concentration of non-converted hydrocarbons in the reaction environment, and consequently deactivates the catalyst. On the other hand, the combustion of the partially structured coke occurs at higher temperature due to the further location of the coke from the metallic sites, thereby hindering its combustion [63, 73]. This type of deposited coke corresponds to the filamentous coke, which generally does not affect directly to catalyst deactivation, as it does not block the active sites [69]. However, when its content is severe, it blocks the active sites, hindering the adsorption of reactants, and consequently increasing the

The aforementioned identification of two types of coke has been corroborated based on the scanning electron microscopy (SEM) image of the deactivated catalyst displayed in **Figure 7**. It should be noted that the nature of the coke deposited on the deactivated catalyst at 123 min reaction is amorphous and fibrillary. Ochoa et al. [74] demonstrated that coke content evolves with time on stream. In this evolution, both types of cokes growth throughout time on stream with different rates, with the one for filamentous coke being higher. However, it can be concluded that coke deposition is more influenced by the growth of encapsulating coke, as has also been

Approximately 40% of the post-consumption wastes come from agriculture, construction, automotive and distribution sectors, and the remaining 60% from municipal solid wastes (MSW). Although the plastics only account for 7 wt% in the MSW, its contribution is 20 vol% of the total MSW volume. Therefore, the

concentration of non-converted hydrocarbons in the reaction medium.

encapsulating coke, which is deposited on the Ni metal.

**80**

**Figure 7.**

*SEM image of the deactivated catalyst.*

between the results for PP and PS are small. However, the most used catalysts in reforming processes are those based on Ni and Co, due mainly to its low cost in relation to noble metals.

**Figure 8b** shows the product yields obtained in the reforming of plastic pyrolysis volatiles. It should be noted that the hydrogen yield is based on the maximum allowable by stoichiometry, but those of the other compounds are given by C mole unit fed into the reforming step. As observed, there is a considerable effect on H2, CO2 and CO yields. On the one hand, the product yields are similar for HDPE and PP, as a consequence of the similar composition of the pyrolysis volatiles to be reformed, with hydrogen yields being 85.7 for HDPE and 83.3% for PP, respectively, and CO2 yields of 67.4 and 64.6% and CO yields of 29.3 and 30.9%, respectively.

However, the distribution of the reforming products is different in the case of PET due to the differences in the pyrolysis volatile stream, with CO2 and CO yields being of 29.3 and 9.9%, respectively. Thus, the product distribution in the reforming step is as follows: hydrogen yield 94.1%, CO2 yield 89.2% and CO yield 10.8%. The high hydrogen yield and low CO yield obtained allow discarding the hypothesis that the origin of the CO2 is the thermal decomposition of the oxygenate compounds. It is in fact produced by the WGS reaction, which is enhanced by the higher value of the effective space time (by carbon atom unit) for this plastic. In addition, it should be noted that yields of CH4, C2▬C4 hydrocarbons and non-converted C5+ are lower than in the case of HDPE and PP, which is a consequence of the higher effective space time used with this plastic.

On the other hand, the hydrogen yield obtained when PS is fed is similar to that obtained in the cases of HDPE and PP, whereas the CO2 yield is slightly lower (60.2%) and that of CO slightly higher (39.8%). This result may also be associated with the lower extent of the WGS reaction due to the lower effective space time used in the case of this plastic.

It should also be pointed out that the results obtained for the PP and HDPE are similar to those obtained in the literature using Ru catalysts [29, 30], although they are obtained at lower temperatures (630 vs. 700°C) and using lower space time values (9.8 vs. 16.7 gcatalyst min gplastic<sup>−</sup><sup>1</sup> ).

#### **4. Conclusions**

The hydrogen production from plastic has been studied in a two-step process. The first is the polymer fast pyrolysis and the second the catalytic steam reforming of pyrolysis volatiles. The process has been developed in a bench scale unit operating in continuous regime. The conical spouted bed reactor has been selected for the pyrolysis step because its features avoid operational problems and allow operating at low pyrolysis temperatures (500°C), minimizing the energy requirement. It has been observed that the yields and the composition of pyrolysis volatiles obtained at 500°C feeding steam are similar to those corresponding to the pyrolysis under N2 atmosphere.

The temperature, space time and steam/plastic ratio in the reforming step have a great influence on the product yields and distributions obtained. An increase in the three variables favors the reforming of the pyrolysis volatiles, obtaining a hydrogen yield of 92.5% of that allowable by stoichiometry for a space time of 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> at 700°C when a steam/plastic ratio of 5 is used. An increase in temperature in the 600– 700°C range increases the conversion from 94.5 to 98.1% and the hydrogen yield from 78.1 to 85.7%. However, the WGS reaction is hindered, which increases the CO yield. An increase in space time causes a considerable increase in the conversion and yields of H2, CO2 and CO, and a decrease in the yields of CH4, C2▬C4 and C5+ hydrocarbons.

**83**

**Author details**

(UPV/EHU), Bilbao, Spain

provided the original work is properly cited.

© 2019 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium,

Itsaso Barbarias, Aitor Arregi, Maite Artetxe, Laura Santamaria, Gartzen Lopez\*,

María Cortazar, Maider Amutio, Javier Bilbao and Martin Olazar

The authors of this chapter declare no conflict of interest.

\*Address all correspondence to: gartzen.lopez@ehu.es

Department of Chemical Engineering, University of the Basque Country

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

hydrocarbons (C2▬C4) and C5+ fraction) increase with time on stream.

Moreover, an increase in the steam/plastic ratio increases the hydrogen yield, by displacing the reforming and the WGS reactions. The conversion obtained with a steam/ plastic ratio of 5 at 700°C and with a space time of 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

The use of a fluidized bed reactor in the reforming step allows the operation without problems. However, reaction rate decreases due to the deposition of coke on the catalyst. As a result of this deposition, the specific surface and pore volume of the catalyst decrease and the yields of non-reformed hydrocarbons (CH4, light

The individual valorization of the different plastics leads to conversion values above 98% in all cases. The reforming behavior is similar for HDPE and PP. PET leads to higher yields of H2 (94.1%) and CO2 (89.2%). In the case of PS, H2 yield is similar to those obtained when HDPE and PP (82.5%) are fed, whereas the CO2

This work was carried out with financial support from the Ministry of Economy

and Competitiveness of the Spanish Government (CTQ2016-75535-R and CTQ-2015-69436-R), the European Regional Development Funds (ERDF), the Basque Government (IT748-13) and the University of the Basque Country (UFI 11/39).

is almost full

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

(99.7%), with a hydrogen yield of 92.5%.

yield is slightly lower (60.2%).

**Acknowledgements**

**Conflict of interest**

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

Moreover, an increase in the steam/plastic ratio increases the hydrogen yield, by displacing the reforming and the WGS reactions. The conversion obtained with a steam/ plastic ratio of 5 at 700°C and with a space time of 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup> is almost full (99.7%), with a hydrogen yield of 92.5%.

The use of a fluidized bed reactor in the reforming step allows the operation without problems. However, reaction rate decreases due to the deposition of coke on the catalyst. As a result of this deposition, the specific surface and pore volume of the catalyst decrease and the yields of non-reformed hydrocarbons (CH4, light hydrocarbons (C2▬C4) and C5+ fraction) increase with time on stream.

The individual valorization of the different plastics leads to conversion values above 98% in all cases. The reforming behavior is similar for HDPE and PP. PET leads to higher yields of H2 (94.1%) and CO2 (89.2%). In the case of PS, H2 yield is similar to those obtained when HDPE and PP (82.5%) are fed, whereas the CO2 yield is slightly lower (60.2%).

## **Acknowledgements**

*Recent Advances in Pyrolysis*

relation to noble metals.

effective space time used with this plastic.

used in the case of this plastic.

**4. Conclusions**

atmosphere.

values (9.8 vs. 16.7 gcatalyst min gplastic<sup>−</sup><sup>1</sup>

between the results for PP and PS are small. However, the most used catalysts in reforming processes are those based on Ni and Co, due mainly to its low cost in

**Figure 8b** shows the product yields obtained in the reforming of plastic pyrolysis volatiles. It should be noted that the hydrogen yield is based on the maximum allowable by stoichiometry, but those of the other compounds are given by C mole unit fed into the reforming step. As observed, there is a considerable effect on H2, CO2 and CO yields. On the one hand, the product yields are similar for HDPE and PP, as a consequence of the similar composition of the pyrolysis volatiles to be reformed, with hydrogen yields being 85.7 for HDPE and 83.3% for PP, respectively, and CO2 yields of 67.4 and 64.6% and CO yields of 29.3 and 30.9%, respectively. However, the distribution of the reforming products is different in the case of PET due to the differences in the pyrolysis volatile stream, with CO2 and CO yields being of 29.3 and 9.9%, respectively. Thus, the product distribution in the reforming step is as follows: hydrogen yield 94.1%, CO2 yield 89.2% and CO yield 10.8%. The high hydrogen yield and low CO yield obtained allow discarding the hypothesis that the origin of the CO2 is the thermal decomposition of the oxygenate compounds. It is in fact produced by the WGS reaction, which is enhanced by the higher value of the effective space time (by carbon atom unit) for this plastic. In addition, it should be noted that yields of CH4, C2▬C4 hydrocarbons and non-converted C5+ are lower than in the case of HDPE and PP, which is a consequence of the higher

On the other hand, the hydrogen yield obtained when PS is fed is similar to that obtained in the cases of HDPE and PP, whereas the CO2 yield is slightly lower (60.2%) and that of CO slightly higher (39.8%). This result may also be associated with the lower extent of the WGS reaction due to the lower effective space time

It should also be pointed out that the results obtained for the PP and HDPE are similar to those obtained in the literature using Ru catalysts [29, 30], although they are obtained at lower temperatures (630 vs. 700°C) and using lower space time

The hydrogen production from plastic has been studied in a two-step process. The first is the polymer fast pyrolysis and the second the catalytic steam reforming of pyrolysis volatiles. The process has been developed in a bench scale unit operating in continuous regime. The conical spouted bed reactor has been selected for the pyrolysis step because its features avoid operational problems and allow operating at low pyrolysis temperatures (500°C), minimizing the energy requirement. It has been observed that the yields and the composition of pyrolysis volatiles obtained at 500°C feeding steam are similar to those corresponding to the pyrolysis under N2

The temperature, space time and steam/plastic ratio in the reforming step have a great influence on the product yields and distributions obtained. An increase in the three variables favors the reforming of the pyrolysis volatiles, obtaining a hydrogen yield of 92.5% of that allowable by stoichiometry for a space time of 16.7 gcatalyst min gHDPE<sup>−</sup><sup>1</sup>

700°C when a steam/plastic ratio of 5 is used. An increase in temperature in the 600– 700°C range increases the conversion from 94.5 to 98.1% and the hydrogen yield from 78.1 to 85.7%. However, the WGS reaction is hindered, which increases the CO yield. An increase in space time causes a considerable increase in the conversion and yields of H2, CO2 and CO, and a decrease in the yields of CH4, C2▬C4 and C5+ hydrocarbons.

).

**82**

This work was carried out with financial support from the Ministry of Economy and Competitiveness of the Spanish Government (CTQ2016-75535-R and CTQ-2015-69436-R), the European Regional Development Funds (ERDF), the Basque Government (IT748-13) and the University of the Basque Country (UFI 11/39).

## **Conflict of interest**

The authors of this chapter declare no conflict of interest.

## **Author details**

Itsaso Barbarias, Aitor Arregi, Maite Artetxe, Laura Santamaria, Gartzen Lopez\*, María Cortazar, Maider Amutio, Javier Bilbao and Martin Olazar Department of Chemical Engineering, University of the Basque Country (UPV/EHU), Bilbao, Spain

\*Address all correspondence to: gartzen.lopez@ehu.es

© 2019 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

at

## **References**

[1] Arregi A, Amutio M, Lopez G, Bilbao J, Olazar M. Evaluation of thermochemical routes for hydrogen production from biomass: A review. Energy Conversion and Management. 2018;**165**:696-719. DOI: 10.1016/j. enconman.2018.03.089

[2] International Energy Agency (IEA). Technology Roadmap: Hydrogen and Fuel Cells; Paris. 2015

[3] Turner J, Sverdrup G, Mann MK, Maness P, Kroposki B, Ghirardi M, et al. Renewable hydrogen production. International Journal of Energy Research. 2008;**32**:379-407. DOI: 10.1002/er.1372

[4] Balat H, Kirtay E. Hydrogen from biomass—Present scenario and future prospects. International Journal of Hydrogen Energy. 2010;**35**:7416-7426. DOI: 10.1016/j.ijhydene.2010.04.137

[5] Trane R, Dahl S, Skjoth-Rasmussen MS, Jensen AD. Catalytic steam reforming of bio-oil. International Journal of Hydrogen Energy. 2012;**37**:6447-6472. DOI: 10.1016/j. ijhydene.2012.01.023

[6] Lopez G, Artetxe M, Amutio M, Alvarez J, Bilbao J, Olazar M. Recent advances in the gasification of waste plastics. A critical overview. Renewable and Sustainable Energy Reviews. 2018;**82**:576-596. DOI: 10.1016/j. rser.2017.09.032

[7] Xiao R, Jin B, Zhou H, Zhong Z, Zhang M. Air gasification of polypropylene plastic waste in fluidized bed gasifier. Energy Conversion and Management. 2007;**48**:778-786. DOI: 10.1016/j.enconman.2006.09.004

[8] Arena U, Di Gregorio F, Amorese C, Mastellone ML. A techno-economic comparison of fluidized bed gasification of two mixed plastic wastes. Waste Management. 2011;**31**:1494-1504

[9] Arena U, Di Gregorio F. Energy generation by air gasification of two industrial plastic wastes in a pilot scale fluidized bed reactor. Energy. 2014;**68**:735-743. DOI: 10.1016/j. energy.2014.01.084

[10] Cho M, Mun T, Choi Y, Kim J. Twostage air gasification of mixed plastic waste: Olivine as the bed material and effects of various additives and a nickelplated distributor on the tar removal. Energy. 2014;**70**:128-134. DOI: 10.1016/j. energy.2014.03.097

[11] Toledo JM, Aznar MP, Sancho JA. Catalytic air gasification of plastic waste (polypropylene) in a fluidized bed. Part II: Effects of some operating variables on the quality of the raw gas produced using olivine as the in-bed material. Industrial and Engineering Chemistry Research. 2011;**50**: 11815-11821. DOI: 10.1021/ie071023q

[12] Jeong Y, Choi Y, Kim J. Three-stage air gasification of waste polyethylene: In-situ regeneration of active carbon used as a tar removal additive. Energy. 2019;**166**:335-342. DOI: 10.1016/j. energy.2018.10.086

[13] Wilk V, Hofbauer H. Conversion of mixed plastic wastes in a dual fluidized bed steam gasifier. Fuel. 2013;**107**: 787-799. DOI: 10.1016/j.fuel.2013.01.068

[14] Kern SJ, Pfeifer C, Hofbauer H. Cogasification of polyethylene and lignite in a dual fluidized bed gasifier. Industrial and Engineering Chemistry Research. 2013;**52**:4360-4371

[15] Wilk V, Hofbauer H. Co-gasification of plastics and biomass in a dual fluidizedbed steam gasifier: Possible interactions of fuels. Energy and Fuels. 2013;**27**:3261- 3273. DOI: 10.1021/ef400349k

[16] Friengfung P, Jamkrajang E, Sunphorka S, Kuchonthara P, Mekasut L.

**85**

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

GV, et al. Novel three-phase steamair plasma torch for gasification of high-caloric waste. Applied Energy. 2013;**108**:505-514. DOI: 10.1016/j.

[24] Hlina M, Hrabovsky M, Kavka T, Konrad M. Production of high quality syngas from argon/water plasma gasification of biomass and waste. Waste Management. 2014;**34**:63-66. DOI: 10.1016/j.wasman.2013.09.018

[25] Wu C, Williams PT. A novel Ni-Mg-Al-CaO catalyst with the dual functions of catalysis and CO2 sorption for H2 production from the pyrolysisgasification of polypropylene. Fuel. 2010;**89**:1435-1441. DOI: 10.1016/j.

[26] Wu C, Williams PT. Investigation of coke formation on Ni-Mg-Al catalyst for hydrogen production from the catalytic steam pyrolysisgasification of polypropylene. Applied Catalysis B: Environmental. 2010;**96**:198-207. DOI: 10.1016/j.

[27] Wu C, Williams PT. Investigation of Ni-Al, Ni-Mg-Al and Ni-Cu-Al catalyst for hydrogen production from pyrolysis-gasification of polypropylene. Applied Catalysis B: Environmental. 2009;**90**:147-156. DOI: 10.1016/j.

[28] Saad JM, Williams PT. Pyrolysiscatalytic-dry reforming of waste plastics and mixed waste plastics for syngas production. Energy and Fuels. 2016;**30**:3198-3204. DOI: 10.1021/acs.

[29] Namioka T, Saito A, Inoue Y, Park Y, Min TJ, Roh SA, et al. Hydrogen-rich gas production from waste plastics by pyrolysis and lowtemperature steam reforming over a ruthenium catalyst. Applied Energy. 2011;**88**:2019-2026. DOI: 10.1016/j.

apenergy.2013.03.052

fuel.2009.10.020

apcatb.2010.02.022

apcatb.2009.03.004

energyfuels.5b02508

apenergy.2010.12.053

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

gasification of different plastics and their mixtures. Industrial and Engineering Chemistry Research. 2014;**53**:1909-1915.

[17] Baloch HA, Yang T, Li R, Nizamuddin S, Kai X, Bhutto AW. Parametric study of co-gasification of ternary blends of rice straw, polyethylene and polyvinylchloride. Clean Technologies and Environmental Policy. 2016;**18**:1031-1042. DOI: 10.1007/

[18] Ahmed II, Gupta AK. Hydrogen production from polystyrene pyrolysis and gasification: Characteristics and kinetics. International Journal of Hydrogen Energy. 2009;**34**:6253-6264. DOI: 10.1016/j.ijhydene.2009.05.046

[19] Guo X, Zhang W, Wang L, Hao J. Comparative study of nitrogen migration among the products from catalytic pyrolysis and gasification of waste rigid polyurethane foam. Journal of Analytical and Applied Pyrolysis. 2016;**120**:144-153. DOI: 10.1016/j.

[20] Erkiaga A, Lopez G, Amutio M, Bilbao J, Olazar M. Syngas from steam gasification of polyethylene in a conical spouted bed reactor. Fuel. 2013;**109**: 461-469. DOI: 10.1016/j.fuel.2013.03.022

[21] Lopez G, Erkiaga A, Artetxe M, Amutio M, Bilbao J, Olazar M. Hydrogen production by high density polyethylene steam gasification and in-line volatile reforming. Industrial and Engineering Chemistry Research. 2015;**54**:9536-9544.

DOI: 10.1021/acs.iecr.5b02413

[22] Lopez G, Erkiaga A, Amutio M, Bilbao J, Olazar M. Effect of polyethylene co-feeding in the steam gasification of biomass in a conical spouted bed reactor. Fuel. 2015;**153**:393- 401. DOI: 10.1016/j.fuel.2015.03.006

[23] Rutberg PG, Kuznetsov VA, Serba EO, Popov SD, Surov AV, Nakonechny

NiO/dolomite catalyzed steam/O2

DOI: 10.1021/ie401893s

s10098-016-1092-4

jaap.2016.04.018

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

NiO/dolomite catalyzed steam/O2 gasification of different plastics and their mixtures. Industrial and Engineering Chemistry Research. 2014;**53**:1909-1915. DOI: 10.1021/ie401893s

[17] Baloch HA, Yang T, Li R, Nizamuddin S, Kai X, Bhutto AW. Parametric study of co-gasification of ternary blends of rice straw, polyethylene and polyvinylchloride. Clean Technologies and Environmental Policy. 2016;**18**:1031-1042. DOI: 10.1007/ s10098-016-1092-4

[18] Ahmed II, Gupta AK. Hydrogen production from polystyrene pyrolysis and gasification: Characteristics and kinetics. International Journal of Hydrogen Energy. 2009;**34**:6253-6264. DOI: 10.1016/j.ijhydene.2009.05.046

[19] Guo X, Zhang W, Wang L, Hao J. Comparative study of nitrogen migration among the products from catalytic pyrolysis and gasification of waste rigid polyurethane foam. Journal of Analytical and Applied Pyrolysis. 2016;**120**:144-153. DOI: 10.1016/j. jaap.2016.04.018

[20] Erkiaga A, Lopez G, Amutio M, Bilbao J, Olazar M. Syngas from steam gasification of polyethylene in a conical spouted bed reactor. Fuel. 2013;**109**: 461-469. DOI: 10.1016/j.fuel.2013.03.022

[21] Lopez G, Erkiaga A, Artetxe M, Amutio M, Bilbao J, Olazar M. Hydrogen production by high density polyethylene steam gasification and in-line volatile reforming. Industrial and Engineering Chemistry Research. 2015;**54**:9536-9544. DOI: 10.1021/acs.iecr.5b02413

[22] Lopez G, Erkiaga A, Amutio M, Bilbao J, Olazar M. Effect of polyethylene co-feeding in the steam gasification of biomass in a conical spouted bed reactor. Fuel. 2015;**153**:393- 401. DOI: 10.1016/j.fuel.2015.03.006

[23] Rutberg PG, Kuznetsov VA, Serba EO, Popov SD, Surov AV, Nakonechny GV, et al. Novel three-phase steamair plasma torch for gasification of high-caloric waste. Applied Energy. 2013;**108**:505-514. DOI: 10.1016/j. apenergy.2013.03.052

[24] Hlina M, Hrabovsky M, Kavka T, Konrad M. Production of high quality syngas from argon/water plasma gasification of biomass and waste. Waste Management. 2014;**34**:63-66. DOI: 10.1016/j.wasman.2013.09.018

[25] Wu C, Williams PT. A novel Ni-Mg-Al-CaO catalyst with the dual functions of catalysis and CO2 sorption for H2 production from the pyrolysisgasification of polypropylene. Fuel. 2010;**89**:1435-1441. DOI: 10.1016/j. fuel.2009.10.020

[26] Wu C, Williams PT. Investigation of coke formation on Ni-Mg-Al catalyst for hydrogen production from the catalytic steam pyrolysisgasification of polypropylene. Applied Catalysis B: Environmental. 2010;**96**:198-207. DOI: 10.1016/j. apcatb.2010.02.022

[27] Wu C, Williams PT. Investigation of Ni-Al, Ni-Mg-Al and Ni-Cu-Al catalyst for hydrogen production from pyrolysis-gasification of polypropylene. Applied Catalysis B: Environmental. 2009;**90**:147-156. DOI: 10.1016/j. apcatb.2009.03.004

[28] Saad JM, Williams PT. Pyrolysiscatalytic-dry reforming of waste plastics and mixed waste plastics for syngas production. Energy and Fuels. 2016;**30**:3198-3204. DOI: 10.1021/acs. energyfuels.5b02508

[29] Namioka T, Saito A, Inoue Y, Park Y, Min TJ, Roh SA, et al. Hydrogen-rich gas production from waste plastics by pyrolysis and lowtemperature steam reforming over a ruthenium catalyst. Applied Energy. 2011;**88**:2019-2026. DOI: 10.1016/j. apenergy.2010.12.053

**84**

*Recent Advances in Pyrolysis*

**References**

enconman.2018.03.089

Fuel Cells; Paris. 2015

ijhydene.2012.01.023

rser.2017.09.032

[1] Arregi A, Amutio M, Lopez G, Bilbao J, Olazar M. Evaluation of thermochemical routes for hydrogen production from biomass: A review. Energy Conversion and Management. 2018;**165**:696-719. DOI: 10.1016/j.

[9] Arena U, Di Gregorio F. Energy generation by air gasification of two industrial plastic wastes in a pilot scale fluidized bed reactor. Energy. 2014;**68**:735-743. DOI: 10.1016/j.

[10] Cho M, Mun T, Choi Y, Kim J. Twostage air gasification of mixed plastic waste: Olivine as the bed material and effects of various additives and a nickelplated distributor on the tar removal. Energy. 2014;**70**:128-134. DOI: 10.1016/j.

[11] Toledo JM, Aznar MP, Sancho JA. Catalytic air gasification of plastic waste (polypropylene) in a fluidized bed. Part II: Effects of some operating variables on the quality of the raw gas produced using olivine as the in-bed material. Industrial and Engineering

Chemistry Research. 2011;**50**: 11815-11821. DOI: 10.1021/ie071023q

[12] Jeong Y, Choi Y, Kim J. Three-stage air gasification of waste polyethylene: In-situ regeneration of active carbon used as a tar removal additive. Energy. 2019;**166**:335-342. DOI: 10.1016/j.

[13] Wilk V, Hofbauer H. Conversion of mixed plastic wastes in a dual fluidized bed steam gasifier. Fuel. 2013;**107**: 787-799. DOI: 10.1016/j.fuel.2013.01.068

[14] Kern SJ, Pfeifer C, Hofbauer H. Cogasification of polyethylene and lignite in a dual fluidized bed gasifier. Industrial and Engineering Chemistry

[15] Wilk V, Hofbauer H. Co-gasification of plastics and biomass in a dual fluidizedbed steam gasifier: Possible interactions of fuels. Energy and Fuels. 2013;**27**:3261-

Research. 2013;**52**:4360-4371

3273. DOI: 10.1021/ef400349k

[16] Friengfung P, Jamkrajang E,

Sunphorka S, Kuchonthara P, Mekasut L.

energy.2014.01.084

energy.2014.03.097

energy.2018.10.086

[2] International Energy Agency (IEA). Technology Roadmap: Hydrogen and

[3] Turner J, Sverdrup G, Mann MK, Maness P, Kroposki B, Ghirardi M, et al. Renewable hydrogen production. International Journal of Energy Research. 2008;**32**:379-407. DOI: 10.1002/er.1372

[4] Balat H, Kirtay E. Hydrogen from biomass—Present scenario and future prospects. International Journal of Hydrogen Energy. 2010;**35**:7416-7426. DOI: 10.1016/j.ijhydene.2010.04.137

[5] Trane R, Dahl S, Skjoth-Rasmussen MS, Jensen AD. Catalytic steam reforming of bio-oil. International Journal of Hydrogen Energy. 2012;**37**:6447-6472. DOI: 10.1016/j.

[6] Lopez G, Artetxe M, Amutio M, Alvarez J, Bilbao J, Olazar M. Recent advances in the gasification of waste plastics. A critical overview. Renewable and Sustainable Energy Reviews. 2018;**82**:576-596. DOI: 10.1016/j.

[7] Xiao R, Jin B, Zhou H, Zhong Z, Zhang M. Air gasification of

polypropylene plastic waste in fluidized bed gasifier. Energy Conversion and Management. 2007;**48**:778-786. DOI: 10.1016/j.enconman.2006.09.004

[8] Arena U, Di Gregorio F, Amorese C, Mastellone ML. A techno-economic comparison of fluidized bed gasification of two mixed plastic wastes. Waste Management. 2011;**31**:1494-1504

[30] Park Y, Namioka T, Sakamoto S, Min TJ, Roh SA, Yoshikawa K. Optimum operating conditions for a twostage gasification process fueled by polypropylene by means of continuous reactor over ruthenium catalyst. Fuel Processing Technology. 2010;**91**:951-957. DOI: 10.1016/j.fuproc.2009.10.014

[31] Czernik S, French RJ. Production of hydrogen from plastics by pyrolysis and catalytic steam reform. Energy and Fuels. 2006;**20**:754-758. DOI: 10.1016/j. fuproc.2009.10.014

[32] Erkiaga A, Lopez G, Barbarias I, Artetxe M, Amutio M, Bilbao J, et al. HDPE pyrolysis-steam reforming in a tandem spouted bed-fixed bed reactor for H2 production. Journal of Analytical and Applied Pyrolysis. 2015;**116**:34-41. DOI: 10.1016/j.jaap.2015.10.010

[33] Barbarias I, Lopez G, Alvarez J, Artetxe M, Arregi A, Bilbao J, et al. A sequential process for hydrogen production based on continuous HDPE fast pyrolysis and in-line steam reforming. Chemical Engineering Journal. 2016;**296**:191-198. DOI: 10.1016/j.cej.2016.03.091

[34] Barbarias I, Lopez G, Artetxe M, Arregi A, Santamaria L, Bilbao J, et al. Pyrolysis and in-line catalytic steam reforming of polystyrene through a twostep reaction system. Journal of Analytical and Applied Pyrolysis. 2016;**122**:502-510. DOI: 10.1016/j.jaap.2016.10.006

[35] Barbarias I, Lopez G, Artetxe M, Arregi A, Bilbao J, Olazar M. Valorisation of different waste plastics by pyrolysis and in-line catalytic steam reforming for hydrogen production. Energy Conversion and Management. 2018;**156**:575-584. DOI: 10.1016/j.enconman.2017.11.048

[36] Arregi A, Amutio M, Lopez G, Artetxe M, Alvarez J, Bilbao J, et al. Hydrogen-rich gas production by continuous pyrolysis and in-line

catalytic reforming of pine wood waste and HDPE mixtures. Energy Conversion and Management. 2017;**136**:192-201. DOI: 10.1016/j.enconman.2017.01.008

[37] Al-Salem SM, Lettieri P, Baeyens J. Recycling and recovery routes of plastic solid waste (PSW): A review. Waste Management. 2009;**29**:2625-2643. DOI: 10.1016/j.wasman.2009.06.004

[38] Lopez G, Artetxe M, Amutio M, Bilbao J, Olazar M. Thermochemical routes for the valorization of waste polyolefinic plastics to produce fuels and chemicals. A review. Renewable and Sustainable Energy Reviews. 2017;**73**:346- 368. DOI: 10.1016/j.rser.2017.01.142

[39] Wong SL, Ngadi N, Abdullah TAT, Inuwa IM. Current state and future prospects of plastic waste as source of fuel: A review. Renewable and Sustainable Energy Reviews. 2015;**50**:1167-1180. DOI: 10.1016/j. rser.2015.04.063

[40] Anuar Sharuddin SD, Abnisa F, Wan Daud WMA, Aroua MK. A review on pyrolysis of plastic wastes. Energy Conversion and Management. 2016;**115**:308-326. DOI: 10.1016/j. enconman.2016.02.037

[41] Zhang X, Lei H, Chen S, Wu J. Catalytic co-pyrolysis of lignocellulosic biomass with polymers: A critical review. Green Chemistry. 2016;**18**:4145-4169. DOI: 10.1039/ C6GC00911E

[42] Jung SH, Cho MH, Kang BS, Kim JS. Pyrolysis of a fraction of waste polypropylene and polyethylene for the recovery of BTX aromatics using a fluidized bed reactor. Fuel Processing Technology. 2010;**91**:277-284. DOI: 10.1016/j.fuproc.2009.10.009

[43] Kaminsky W, Predel M, Sadiki A. Feedstock recycling of polymers by pyrolysis in a fluidised bed. Polymer Degradation and Stability.

**87**

ie900557c

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

polyolefin cracking on an HZSM-5

spouted bed reactor. Industrial and Engineering Chemistry Research. 2011;**50**:6061-6070. DOI: 10.1021/

[51] Lopez G, Alvarez J, Amutio M, Mkhize NM, Danon B, van der Gryp P, et al. Waste truck-tyre processing by flash pyrolysis in a conical spouted bed reactor. Energy Conversion and Management. 2017;**142**:523-532. DOI: 10.1016/j.enconman.2017.03.051

[52] Artetxe M, Lopez G, Amutio M, Barbarias I, Arregi A, Aguado R, et al. Styrene recovery from polystyrene by flash pyrolysis in a conical spouted bed reactor. Waste Management. 2015;**46**:126-133. DOI: 10.1016/j.

[53] Fernandez-Akarregi AR, Makibar J, Lopez G, Amutio M, Olazar M. Design and operation of a conical spouted bed reactor pilot plant (25 kg/h) for biomass fast pyrolysis. Fuel Processing Technology. 2013;**112**:48-56. DOI: 10.1016/j.fuproc.2013.02.022

[54] Makibar J, Fernandez-Akarregi AR, Amutio M, Lopez G, Olazar M. Performance of a conical spouted bed pilot plant for bio-oil production by poplar flash pyrolysis. Fuel Processing Technology. 2015;**137**:283-289. DOI:

10.1016/j.fuproc.2015.03.011

[55] Al-Salem SM, Antelava A, Constantinou A, Manos G, Dutta A. A review on thermal and catalytic pyrolysis of plastic solid waste (PSW). Journal of Environmental Management.

2017;**197**:177-198. DOI: 10.1016/j.

Chandrashekaran SR, Sharma BK. Plastics to fuel: A review. Renewable and Sustainable Energy Reviews. 2016;**54**:421-428. DOI: 10.1016/j.

jenvman.2017.03.084

rser.2015.10.015

[56] Kunwar B, Cheng HN,

wasman.2015.05.034

zeolite catalyst in a conical

ie2002999

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

2004;**85**:1045-1050. DOI: 10.1016/j. polymdegradstab.2003.05.002

[44] Kaminsky W, Schlesselmann B, Simon C. Olefins from polyolefins and mixed plastics by pyrolysis. Journal of Analytical and Applied Pyrolysis. 1995;**32**:19-27. DOI: 10.1016/0165-2370(94)00830-T

[45] Kaminsky W, Schlesselmann B, Simon CM. Thermal degradation of mixed plastic waste to aromatics and gas. Polymer Degradation and Stability. 1996;**53**:189-197. DOI: 10.1016/0141-3910(96)00087-0

[46] Mastellone ML, Arena U. Bed defluidisation during the fluidised bed pyrolysis of plastic waste mixtures. Polymer Degradation and Stability. 2004;**85**:1051-1058. DOI: 10.1016/j. polymdegradstab.2003.04.002

[47] Artetxe M, Lopez G, Amutio M, Elordi G, Olazar M, Bilbao J. Operating conditions for the pyrolysis of poly- (ethylene terephthalate) in a conical spouted-bed reactor. Industrial and Engineering Chemistry Research. 2010;**49**:2064-2069. DOI: 10.1021/

[48] Arabiourrutia M, Elordi G, Lopez G, Borsella E, Bilbao J, Olazar M. Characterization of the waxes obtained by the pyrolysis of polyolefin plastics in a conical spouted bed reactor. Journal of Analytical and Applied Pyrolysis. 2012;**94**:230-237. DOI:

10.1016/j.jaap.2011.12.012

10.1021/ie200186m

[49] Elordi G, Olazar M, Lopez G, Artetxe M, Bilbao J. Product yields and compositions in the continuous pyrolysis of high-density polyethylene in a conical spouted bed reactor. Industrial and Engineering Chemistry Research. 2011;**50**:6650-6659. DOI:

[50] Elordi G, Olazar M, Lopez G, Artetxe M, Bilbao J. Continuous

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

2004;**85**:1045-1050. DOI: 10.1016/j. polymdegradstab.2003.05.002

*Recent Advances in Pyrolysis*

fuproc.2009.10.014

[30] Park Y, Namioka T, Sakamoto S, Min TJ, Roh SA, Yoshikawa K. Optimum catalytic reforming of pine wood waste and HDPE mixtures. Energy Conversion and Management. 2017;**136**:192-201. DOI: 10.1016/j.enconman.2017.01.008

[37] Al-Salem SM, Lettieri P, Baeyens J. Recycling and recovery routes of plastic solid waste (PSW): A review. Waste Management. 2009;**29**:2625-2643. DOI: 10.1016/j.wasman.2009.06.004

[38] Lopez G, Artetxe M, Amutio M, Bilbao J, Olazar M. Thermochemical routes for the valorization of waste polyolefinic plastics to produce fuels and chemicals. A review. Renewable and Sustainable Energy Reviews. 2017;**73**:346- 368. DOI: 10.1016/j.rser.2017.01.142

[39] Wong SL, Ngadi N, Abdullah TAT, Inuwa IM. Current state and future prospects of plastic waste as source of fuel: A review. Renewable and Sustainable Energy Reviews. 2015;**50**:1167-1180. DOI: 10.1016/j.

[40] Anuar Sharuddin SD, Abnisa F, Wan Daud WMA, Aroua MK. A review on pyrolysis of plastic wastes. Energy Conversion and Management. 2016;**115**:308-326. DOI: 10.1016/j.

rser.2015.04.063

enconman.2016.02.037

C6GC00911E

[41] Zhang X, Lei H, Chen S, Wu J. Catalytic co-pyrolysis of

lignocellulosic biomass with polymers: A critical review. Green Chemistry. 2016;**18**:4145-4169. DOI: 10.1039/

[42] Jung SH, Cho MH, Kang BS, Kim JS. Pyrolysis of a fraction of waste polypropylene and polyethylene for the recovery of BTX aromatics using a fluidized bed reactor. Fuel Processing Technology. 2010;**91**:277-284. DOI: 10.1016/j.fuproc.2009.10.009

[43] Kaminsky W, Predel M, Sadiki A. Feedstock recycling of polymers by pyrolysis in a fluidised bed. Polymer Degradation and Stability.

[31] Czernik S, French RJ. Production of hydrogen from plastics by pyrolysis and catalytic steam reform. Energy and Fuels. 2006;**20**:754-758. DOI: 10.1016/j.

[32] Erkiaga A, Lopez G, Barbarias I, Artetxe M, Amutio M, Bilbao J, et al. HDPE pyrolysis-steam reforming in a tandem spouted bed-fixed bed reactor for H2 production. Journal of Analytical and Applied Pyrolysis. 2015;**116**:34-41.

DOI: 10.1016/j.jaap.2015.10.010

10.1016/j.cej.2016.03.091

[33] Barbarias I, Lopez G, Alvarez J, Artetxe M, Arregi A, Bilbao J, et al. A sequential process for hydrogen production based on continuous HDPE fast pyrolysis and in-line steam reforming. Chemical Engineering Journal. 2016;**296**:191-198. DOI:

[34] Barbarias I, Lopez G, Artetxe M, Arregi A, Santamaria L, Bilbao J, et al. Pyrolysis and in-line catalytic steam reforming of polystyrene through a twostep reaction system. Journal of Analytical and Applied Pyrolysis. 2016;**122**:502-510.

DOI: 10.1016/j.jaap.2016.10.006

[35] Barbarias I, Lopez G, Artetxe M, Arregi A, Bilbao J, Olazar M. Valorisation of different waste plastics by pyrolysis and in-line

catalytic steam reforming for hydrogen production. Energy Conversion and Management. 2018;**156**:575-584. DOI: 10.1016/j.enconman.2017.11.048

[36] Arregi A, Amutio M, Lopez G, Artetxe M, Alvarez J, Bilbao J, et al. Hydrogen-rich gas production by continuous pyrolysis and in-line

operating conditions for a twostage gasification process fueled by polypropylene by means of continuous reactor over ruthenium catalyst. Fuel Processing Technology. 2010;**91**:951-957. DOI: 10.1016/j.fuproc.2009.10.014

**86**

[44] Kaminsky W, Schlesselmann B, Simon C. Olefins from polyolefins and mixed plastics by pyrolysis. Journal of Analytical and Applied Pyrolysis. 1995;**32**:19-27. DOI: 10.1016/0165-2370(94)00830-T

[45] Kaminsky W, Schlesselmann B, Simon CM. Thermal degradation of mixed plastic waste to aromatics and gas. Polymer Degradation and Stability. 1996;**53**:189-197. DOI: 10.1016/0141-3910(96)00087-0

[46] Mastellone ML, Arena U. Bed defluidisation during the fluidised bed pyrolysis of plastic waste mixtures. Polymer Degradation and Stability. 2004;**85**:1051-1058. DOI: 10.1016/j. polymdegradstab.2003.04.002

[47] Artetxe M, Lopez G, Amutio M, Elordi G, Olazar M, Bilbao J. Operating conditions for the pyrolysis of poly- (ethylene terephthalate) in a conical spouted-bed reactor. Industrial and Engineering Chemistry Research. 2010;**49**:2064-2069. DOI: 10.1021/ ie900557c

[48] Arabiourrutia M, Elordi G, Lopez G, Borsella E, Bilbao J, Olazar M. Characterization of the waxes obtained by the pyrolysis of polyolefin plastics in a conical spouted bed reactor. Journal of Analytical and Applied Pyrolysis. 2012;**94**:230-237. DOI: 10.1016/j.jaap.2011.12.012

[49] Elordi G, Olazar M, Lopez G, Artetxe M, Bilbao J. Product yields and compositions in the continuous pyrolysis of high-density polyethylene in a conical spouted bed reactor. Industrial and Engineering Chemistry Research. 2011;**50**:6650-6659. DOI: 10.1021/ie200186m

[50] Elordi G, Olazar M, Lopez G, Artetxe M, Bilbao J. Continuous

polyolefin cracking on an HZSM-5 zeolite catalyst in a conical spouted bed reactor. Industrial and Engineering Chemistry Research. 2011;**50**:6061-6070. DOI: 10.1021/ ie2002999

[51] Lopez G, Alvarez J, Amutio M, Mkhize NM, Danon B, van der Gryp P, et al. Waste truck-tyre processing by flash pyrolysis in a conical spouted bed reactor. Energy Conversion and Management. 2017;**142**:523-532. DOI: 10.1016/j.enconman.2017.03.051

[52] Artetxe M, Lopez G, Amutio M, Barbarias I, Arregi A, Aguado R, et al. Styrene recovery from polystyrene by flash pyrolysis in a conical spouted bed reactor. Waste Management. 2015;**46**:126-133. DOI: 10.1016/j. wasman.2015.05.034

[53] Fernandez-Akarregi AR, Makibar J, Lopez G, Amutio M, Olazar M. Design and operation of a conical spouted bed reactor pilot plant (25 kg/h) for biomass fast pyrolysis. Fuel Processing Technology. 2013;**112**:48-56. DOI: 10.1016/j.fuproc.2013.02.022

[54] Makibar J, Fernandez-Akarregi AR, Amutio M, Lopez G, Olazar M. Performance of a conical spouted bed pilot plant for bio-oil production by poplar flash pyrolysis. Fuel Processing Technology. 2015;**137**:283-289. DOI: 10.1016/j.fuproc.2015.03.011

[55] Al-Salem SM, Antelava A, Constantinou A, Manos G, Dutta A. A review on thermal and catalytic pyrolysis of plastic solid waste (PSW). Journal of Environmental Management. 2017;**197**:177-198. DOI: 10.1016/j. jenvman.2017.03.084

[56] Kunwar B, Cheng HN, Chandrashekaran SR, Sharma BK. Plastics to fuel: A review. Renewable and Sustainable Energy Reviews. 2016;**54**:421-428. DOI: 10.1016/j. rser.2015.10.015

[57] Wu C, Williams PT. Pyrolysisgasification of post-consumer municipal solid plastic waste for hydrogen production. International Journal of Hydrogen Energy. 2010;**35**:949-957. DOI: 10.1016/j.ijhydene.2009.11.045

[58] Tsuji T, Hatayama A. Gasification of waste plastics by steam reforming in a fluidized bed. Journal of Material Cycles and Waste Management. 2009;**11**:144-147. DOI: 10.1007/s10163-008-0227-z

[59] Luo S, Zhou Y, Yi C. Syngas production by catalytic steam gasification of municipal solid waste in fixed-bed reactor. Energy. 2012;**44**:391-395. DOI: 10.1016/j.energy.2012.06.016

[60] Wu C, Williams PT. Effects of gasification temperature and catalyst ratio on hydrogen production from catalytic steam pyrolysis-gasification of polypropylene. Energy and Fuels. 2008;**22**:4125-4132. DOI: 10.1021/ ef800574w

[61] Wang J, Cheng G, You Y, Xiao B, Liu S, He P, et al. Hydrogen-rich gas production by steam gasification of municipal solid waste (MSW) using NiO supported on modified dolomite. International Journal of Hydrogen Energy. 2012;**37**:6503-6510. DOI: 10.1016/j.ijhydene.2012.01.070

[62] Li J, Liao S, Dan W, Jia K, Zhou X. Experimental study on catalytic steam gasification of municipal solid waste for bioenergy production in a combined fixed bed reactor. Biomass and Bioenergy. 2012;**46**:174-180. DOI: 10.1016/j.biombioe.2012.08.026

[63] Acomb JC, Wu C, Williams PT. Control of steam input to the pyrolysis-gasification of waste plastics for improved production of hydrogen or carbon nanotubes. Applied Catalysis B: Environmental. 2014;**147**:571-584. DOI: 10.1016/j.apcatb.2013.09.018

[64] Wu C, Williams PT. Hydrogen production from the pyrolysis/ gasification of polypropylene: Influence of steam flow rate, carrier gas flow rate and gasification temperature. Energy and Fuels. 2009;**23**:5055-5061. DOI: 10.1021/ef900278w

[65] Wu C, Williams PT. Pyrolysisgasification of plastics, mixed plastics and real-world plastic waste with and without Ni-Mg-Al catalyst. Fuel. 2010;**89**:3022-3032. DOI: 10.1016/j. fuel.2010.05.032

[66] Donatelli A, Iovane P, Molino A. High energy syngas production by waste tyres steam gasification in a rotary kiln pilot plant. Experimental and numerical investigations. Fuel. 2010;**89**:2721-2728. DOI: 10.1016/j. fuel.2010.03.040

[67] Barbarias I, Artetxe M, Lopez G, Arregi A, Bilbao J, Olazar M. Influence of the conditions for reforming HDPE pyrolysis volatiles on the catalyst deactivation by coke. Fuel Processing Technology. 2018;**171**:100-109. DOI: 10.1016/j.fuproc.2017.11.003

[68] Remiro A, Valle B, Aguayo AT, Bilbao J, Gayubo AG. Operating conditions for attenuating Ni/La2O3- Al2O3 catalyst deactivation in the steam reforming of bio-oil aqueous fraction. Fuel Processing Technology. 2013;**115**:222-232. DOI: 10.1016/j. fuproc.2013.06.003

[69] Vicente J, Montero C, Ereña J, Azkoiti MJ, Bilbao J, Gayubo AG. Coke deactivation of Ni and Co catalysts in ethanol steam reforming at mild temperatures in a fluidized bed reactor. International Journal of Hydrogen Energy. 2014;**39**:12586-12596. DOI: 10.1016/j.ijhydene.2014.06.093

[70] Rostrup-Nielsen JR, Sehested J. Whisker carbon revisited. Studies

**89**

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming…*

*DOI: http://dx.doi.org/10.5772/intechopen.85048*

in Surface Science and Catalysis. 2001;**139**:1-12. DOI: 10.1016/ S0167-2991(01)80174-9

[71] Joensen F, Rostrup-Nielsen JR. Conversion of hydrocarbons and alcohols for fuel cells. Journal of Power Sources. 2002;**105**:195-201. DOI: 10.1016/S0378-7753(01)00939-9

cattod.2014.05.043

apcatb.2017.02.015

jcat.2015.08.005

[72] Angeli SD, Pilitsis FG, Lemonidou AA. Methane steam reforming at low temperature: Effect of light alkanes' presence on coke formation. Catalysis Today. 2015:119-128. DOI: 10.1016/j.

[73] Barbarias I, Lopez G, Amutio M, Artetxe M, Alvarez J, Arregi A, et al. Steam reforming of plastic pyrolysis model hydrocarbons and catalyst deactivation. Applied Catalysis A: General. 2016;**527**:152-160. DOI: 10.1016/j.apcata.2016.09.003

[74] Ochoa A, Barbarias I, Artetxe M, Gayubo AG, Olazar M, Bilbao J, et al. Deactivation dynamics of a Ni supported catalyst during the steam reforming of volatiles from waste polyethylene pyrolysis. Applied Catalysis B: Environmental. 2017;**209**:554-565. DOI: 10.1016/j.

[75] Montero C, Ochoa A, Castaño P, Bilbao J, Gayubo AG. Monitoring NiO and coke evolution during the deactivation of a Ni/La2O3-αAl2O3 catalyst in ethanol steam reforming in a fluidized bed. Journal of Catalysis. 2015;**331**:181-192. DOI: 10.1016/j.

[76] Trimm DL. Coke formation and minimisation during steam reforming reactions. Catalysis Today. 1997;**37**:233. DOI: 10.1016/S0920-5861(97)00014-X

*Waste Plastics Valorization by Fast Pyrolysis and in Line Catalytic Steam Reforming… DOI: http://dx.doi.org/10.5772/intechopen.85048*

in Surface Science and Catalysis. 2001;**139**:1-12. DOI: 10.1016/ S0167-2991(01)80174-9

*Recent Advances in Pyrolysis*

[57] Wu C, Williams PT. Pyrolysisgasification of post-consumer municipal [64] Wu C, Williams PT. Hydrogen production from the pyrolysis/

[65] Wu C, Williams PT. Pyrolysisgasification of plastics, mixed plastics and real-world plastic waste with and without Ni-Mg-Al catalyst. Fuel. 2010;**89**:3022-3032. DOI: 10.1016/j.

[66] Donatelli A, Iovane P, Molino A. High energy syngas production by waste tyres steam gasification in a rotary kiln pilot plant. Experimental and numerical investigations. Fuel. 2010;**89**:2721-2728. DOI: 10.1016/j.

[67] Barbarias I, Artetxe M, Lopez G, Arregi A, Bilbao J, Olazar M. Influence of the conditions for reforming HDPE pyrolysis volatiles on the catalyst deactivation by coke. Fuel Processing Technology. 2018;**171**:100-109. DOI:

10.1016/j.fuproc.2017.11.003

fuproc.2013.06.003

[68] Remiro A, Valle B, Aguayo AT, Bilbao J, Gayubo AG. Operating conditions for attenuating Ni/La2O3- Al2O3 catalyst deactivation in the steam reforming of bio-oil aqueous fraction. Fuel Processing Technology. 2013;**115**:222-232. DOI: 10.1016/j.

[69] Vicente J, Montero C, Ereña J, Azkoiti MJ, Bilbao J, Gayubo AG. Coke deactivation of Ni and Co catalysts in ethanol steam reforming at mild temperatures in a fluidized bed reactor. International Journal of Hydrogen Energy. 2014;**39**:12586-12596. DOI: 10.1016/j.ijhydene.2014.06.093

[70] Rostrup-Nielsen JR, Sehested J. Whisker carbon revisited. Studies

10.1021/ef900278w

fuel.2010.05.032

fuel.2010.03.040

gasification of polypropylene: Influence of steam flow rate, carrier gas flow rate and gasification temperature. Energy and Fuels. 2009;**23**:5055-5061. DOI:

[58] Tsuji T, Hatayama A. Gasification of waste plastics by steam reforming in a fluidized bed. Journal of Material Cycles and Waste Management. 2009;**11**:144-147.

DOI: 10.1007/s10163-008-0227-z

[59] Luo S, Zhou Y, Yi C. Syngas

[60] Wu C, Williams PT. Effects of gasification temperature and catalyst ratio on hydrogen production from catalytic steam pyrolysis-gasification of polypropylene. Energy and Fuels. 2008;**22**:4125-4132. DOI: 10.1021/

[61] Wang J, Cheng G, You Y, Xiao B, Liu S, He P, et al. Hydrogen-rich gas production by steam gasification of municipal solid waste (MSW) using NiO supported on modified dolomite. International Journal of Hydrogen Energy. 2012;**37**:6503-6510. DOI: 10.1016/j.ijhydene.2012.01.070

[62] Li J, Liao S, Dan W, Jia K, Zhou X. Experimental study on catalytic steam gasification of municipal solid waste for bioenergy production in a combined fixed bed reactor. Biomass and Bioenergy. 2012;**46**:174-180. DOI: 10.1016/j.biombioe.2012.08.026

[63] Acomb JC, Wu C, Williams PT. Control of steam input to the pyrolysis-gasification of waste plastics for improved production of hydrogen or carbon nanotubes. Applied Catalysis B: Environmental. 2014;**147**:571-584. DOI:

10.1016/j.apcatb.2013.09.018

ef800574w

production by catalytic steam gasification of municipal solid waste in fixed-bed reactor. Energy. 2012;**44**:391-395. DOI: 10.1016/j.energy.2012.06.016

solid plastic waste for hydrogen production. International Journal of Hydrogen Energy. 2010;**35**:949-957. DOI: 10.1016/j.ijhydene.2009.11.045

**88**

[71] Joensen F, Rostrup-Nielsen JR. Conversion of hydrocarbons and alcohols for fuel cells. Journal of Power Sources. 2002;**105**:195-201. DOI: 10.1016/S0378-7753(01)00939-9

[72] Angeli SD, Pilitsis FG, Lemonidou AA. Methane steam reforming at low temperature: Effect of light alkanes' presence on coke formation. Catalysis Today. 2015:119-128. DOI: 10.1016/j. cattod.2014.05.043

[73] Barbarias I, Lopez G, Amutio M, Artetxe M, Alvarez J, Arregi A, et al. Steam reforming of plastic pyrolysis model hydrocarbons and catalyst deactivation. Applied Catalysis A: General. 2016;**527**:152-160. DOI: 10.1016/j.apcata.2016.09.003

[74] Ochoa A, Barbarias I, Artetxe M, Gayubo AG, Olazar M, Bilbao J, et al. Deactivation dynamics of a Ni supported catalyst during the steam reforming of volatiles from waste polyethylene pyrolysis. Applied Catalysis B: Environmental. 2017;**209**:554-565. DOI: 10.1016/j. apcatb.2017.02.015

[75] Montero C, Ochoa A, Castaño P, Bilbao J, Gayubo AG. Monitoring NiO and coke evolution during the deactivation of a Ni/La2O3-αAl2O3 catalyst in ethanol steam reforming in a fluidized bed. Journal of Catalysis. 2015;**331**:181-192. DOI: 10.1016/j. jcat.2015.08.005

[76] Trimm DL. Coke formation and minimisation during steam reforming reactions. Catalysis Today. 1997;**37**:233. DOI: 10.1016/S0920-5861(97)00014-X

**91**

**Chapter 6**

**Abstract**

**1. Introduction**

rocks [2, 3].

of iron and steel [6–11].

Sumatera

Synthesis and Characterization

Nanomaterials of Dunite from

The topics to be discussed are about the synthesis and characterization of forsterite nanoparticles (Mg2So4) from dunite rocks originating from West Sumatra. This region is a meeting of two Indian and Australian plates that give rise to mineral dunite with unique characteristics. Forsterite synthesis was carried out using calcinations temperature variations namely 700, 800, 900, 1000 and 1100°C. Synthesis of forsterite nanoparticles used the High Energy Milling Ellipse 3D Motion (HEM-E3D) method with variations in milling time, i.e., 5, 10, 20 h. Characterization was carried out using X-Ray Fluorescence (XRF) and X-Ray Diffraction (XRD) and Scanning Electron Microscopy (SEM). The synthesis results explain the forsterite concentration in dunite rock, pure forsterite at optimal calcinations temperature, forsterite nanoparticles at optimal grinding time and forsterite nanoparticle structure.

Forsterite is a magnesium silicate crystal with the chemical formula Mg2SiO4 derived from the olivine mineral group [1]. Olivine is a group of minerals composed of iron (Fe) and magnesium (Mg). The olivine mineral is green, with luster, formed at high temperatures. This mineral is commonly found in basalt and ultramafic rocks. Rocks whose overall minerals consist of olivine minerals are known as dunite

Forsterite is often used as an electronic component because it has a low coefficient of thermal expansion and electrical conductivity [4]. Besides that, forsterite has superior properties, namely chemical stability at high temperatures [5] and high electrical properties so that it can be used as a coating for the back, edges, and front

Iron and steel are widely used in industry and property such as building materi-

als, ships, electronic equipment, etc. But in its use, steel is easily corrosion. To overcome this corrosion problem, a lot of research continues. One of them is by soaking the steel with an anti-corrosion solution. But the results are not yet suitable for achieving commercial applications. The reason is that the particle size of the anti-corrosion powder used is relatively very large, giving rise to new problems,

of Forsterite (Mg2SiO4)

*Ratnawulan Ratnawulan and Ahmad Fauzi*

**Keywords:** forsterite, nanoparticles, dunite, HEM-E3D, milling time

## **Chapter 6**
